
#=======================================================================
data_global
#=======================================================================

_audit_creation_method                   'Jana2006 Version : 13/05/2019'


# 1. PROCESSING SUMMARY (IUCr Office Use Only)

_journal_date_recd_electronic            ?
_journal_date_to_coeditor                ?
_journal_date_from_coeditor              ?
_journal_date_accepted                   ?
_journal_date_printers_first             ?
_journal_date_printers_final             ?
_journal_date_proofs_out                 ?
_journal_date_proofs_in                  ?
_journal_coeditor_name                   ?
_journal_coeditor_code                   ?
_journal_coeditor_notes
; ?
;
_journal_techeditor_code                 ?
_journal_paper_category                  ?
_journal_techeditor_notes
; ?
;
_journal_coden_ASTM                      ?
_journal_name_full                       'Dalton Trans.'
_journal_year                            ?
_journal_volume                          ?
_journal_issue                           ?
_journal_page_first                      ?
_journal_page_last                       ?
_journal_suppl_publ_number               ?
_journal_suppl_publ_pages                ?

#=======================================================================

# 2. SUBMISSION DETAILS

_publ_contact_author_name                'Dr. Oliver Janka'
_publ_contact_author_address     
;Institut für Anorganische und Analytische Chemie
Corrensstrasse 30
48149 Münster
;
_publ_contact_author_email       ocjanka@uni-muenster.de
_publ_contact_author_phone       '0049 251 83-36047'
_publ_contact_author_fax         '0049 251 83-36002'

_publ_requested_journal                  'Dalton Transactions'
_publ_requested_category                 ?

_publ_contact_letter
; ?
;

#=======================================================================

# 3. TITLE AND AUTHOR LIST

_publ_section_title
; ?
;
_publ_section_title_footnote
; ?
;
loop_
 _publ_author_name
 _publ_author_address
      'Frank Stegemann, MSc.'
;      Institut für Anorganische und Analytische Chemie
       Westfälische Wilhelms-Universität Münster
       Corrensstrasse 28/30
       48149 Münster
       Bundesrepublik Deutschland
;
      'Rachid St. Touzani'
;      Institut für Werkstoff- und Fügetechnik (IWF)
       Otto-von-Guericke-Universität Magdeburg
       Grosse Steinernetischstrasse 6
       39104 Magdeburg
       Bundesrepublik Deutschland
;
      'Priv.-Doz. Dr. Oliver Janka'
;      Institut für Anorganische und Analytische Chemie
       Westfälische Wilhelms-Universität Münster
       Corrensstrasse 28/30
       48149 Münster
       Bundesrepublik Deutschland
;
#=======================================================================

# 4. TEXT

_publ_section_synopsis
; ?
;
_publ_section_abstract
; ?
;
_publ_section_comment
; ?
;
_publ_section_introduction
; ?
;
_publ_section_experimental
; ?
;
_publ_section_exptl_prep
; ?
;
_publ_section_exptl_refinement
; ?
;
_publ_section_exptl_solution
; ?
;
_publ_section_discussion
; ?
;
_publ_section_acknowledgements
; ?
;
_publ_section_references
;
Petricek, V., Dusek, M. & Palatinus L. (2014). Z. Kristallogr. 229(5), 345-352.

Palatinus L. & Chapuis G. (2007). J. Appl. Cryst. 40, 786-790.

# enable this reference if Diamond ver. 2 was used for visualization
#Brandenburg, K. (1999). DIAMOND. Version. 2.1c.
#Crystal Impact GbR, Bonn, Germany.

# enable this reference if Diamond ver. 3 was used for visualization
#Brandenburg, K. & Putz, H. (2005). DIAMOND Version 3.
#Crystal Impact GbR, Postfach 1251, D-53002 Bonn, Germany.

# enable this reference if SIR97 was used for solving of the structure
#Altomare, A., Burla, M. C., Camalli, M., Cascarano, G., Giacovazzo, C.,
#Guagliardi, A., Moliterni, A. G. G., Polidori, G., Spagna, R. (1997).
#SIR97. A Package for Crystal Structure Solution by Direct Methods
#and Refinement, Bari, Rome, Italy.

# use this reference if SIR2002 was used for solving of the structure
#Burla, M.C., Camalli, M., Carrozzini, B., Cascarano, G., Giacovazzo, C.,
#Polidori, G., Spagna, R.
#SIR2002: the program, J. Appl. Cryst, (2003). 36, 1103


# use this reference if SIR2011 was used for solving of the structure
#Burla, M.C., Caliandro, R., Camalli, M., Carrozzini, B., Cascarano,
#G.L., Giacovazzo, C., Mallamo. M., Mazzone, A., Polidori, G., Spagna, R.
#SIR2011: a new package for crystal structure determination and refinement,
#J.Appl.Cryst. (2012) 45, 357-361

# enable this reference if bond valences were calculated
#Brown, I. D. (1996). J. Appl. Cryst. 29, 479-480.

# enable this reference if Xshape wase used for crystal shape refinement
#Stoe & Cie (1998). X-SHAPE. Stoe & Cie, Darmstadt, Germany.


# enable this reference if Flack coefficient was refined
#Flack, H. D. (1983). Acta Cryst. A39, 876-881.
;
_publ_section_figure_captions
; ?
;
_publ_section_table_legends
; ?
;

#=======================================================================
data_I
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic
; ?
;
_chemical_name_common                    ?
_chemical_formula_moiety                 ?
_chemical_formula_structural             ?
_chemical_formula_analytical             ?
_chemical_formula_iupac                  ?
_chemical_formula_sum                    'Al53 Ba6 Pt21.92'
_chemical_formula_weight                 6530.2
_chemical_melting_point                  ?
_chemical_compound_source                ?
_chemical_absolute_configuration         .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting                   hexagonal
_symmetry_space_group_name_H-M           'P 63/m c m'
_symmetry_space_group_name_Hall          '-P 6c;-2'
_symmetry_Int_Tables_number              193

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -y,x-y,z
 3   -x+y,-x,z
 4   -x,-y,z+1/2
 5   y,-x+y,z+1/2
 6   x-y,x,z+1/2
 7   y,x,-z+1/2
 8   x-y,-y,-z+1/2
 9   -x,-x+y,-z+1/2
 10  -y,-x,-z
 11  -x+y,y,-z
 12  x,x-y,-z
 13  -x,-y,-z
 14  y,-x+y,-z
 15  x-y,x,-z
 16  x,y,-z+1/2
 17  -y,x-y,-z+1/2
 18  -x+y,-x,-z+1/2
 19  -y,-x,z+1/2
 20  -x+y,y,z+1/2
 21  x,x-y,z+1/2
 22  y,x,z
 23  x-y,-y,z
 24  -x,-x+y,z

_cell_length_a                           14.2621(5)
_cell_length_b                           14.2621(5)
_cell_length_c                           16.1314(6)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        120
_cell_volume                             2841.6

loop_
 _twin_individual_id
 _twin_individual_mass_fraction_refined
 _twin_individual_twin_matrix_11
 _twin_individual_twin_matrix_12
 _twin_individual_twin_matrix_13
 _twin_individual_twin_matrix_21
 _twin_individual_twin_matrix_22
 _twin_individual_twin_matrix_23
 _twin_individual_twin_matrix_31
 _twin_individual_twin_matrix_32
 _twin_individual_twin_matrix_33
 ? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z                    2

_cell_measurement_reflns_used            28059
_cell_measurement_theta_min              1.65
_cell_measurement_theta_max              35.0
_cell_measurement_temperature            285
_cell_special_details
; ?
;

_exptl_crystal_density_diffrn            7.63
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            ?
_exptl_crystal_F_000                     5470

_exptl_absorpt_coefficient_mu            58.6
_exptl_crystal_description               block
_exptl_crystal_size_max                  0.080
_exptl_crystal_size_mid                  0.055
_exptl_crystal_size_min                  0.040
_exptl_crystal_size_rad                  ?
_exptl_crystal_colour                    silver
_exptl_absorpt_correction_type           numerical
_exptl_absorpt_process_details           ?
_exptl_absorpt_correction_T_min          0.040
_exptl_absorpt_correction_T_max          0.170
loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 ? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details                   ?

_diffrn_ambient_temperature              285
_diffrn_source                           ?
_diffrn_source_power                     ?
_diffrn_source_voltage                   ?
_diffrn_source_current                   ?
_diffrn_radiation_type                   'Mo K\a'
_diffrn_radiation_source                 'X-ray tube'
_diffrn_radiation_wavelength             0.71073
_diffrn_radiation_monochromator          graphite
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type          'Stoe StadiVari'
_diffrn_detector                         ?
_diffrn_detector_area_resol_mean         ?
_diffrn_measurement_method               '??integration method??'
_diffrn_measurement_specimen_support     ?

_diffrn_reflns_number                    13214
_diffrn_reflns_theta_min                 2.53
_diffrn_reflns_theta_max                 31
_diffrn_reflns_theta_full                30.96
_diffrn_measured_fraction_theta_max      0.98
_diffrn_measured_fraction_theta_full     0.98
_diffrn_reflns_av_R_equivalents          0.0461
_diffrn_reflns_av_unetI/netI             0.0200
_diffrn_reflns_limit_h_min               -18
_diffrn_reflns_limit_h_max               18
_diffrn_reflns_limit_k_min               -19
_diffrn_reflns_limit_k_max               19
_diffrn_reflns_limit_l_min               -22
_diffrn_reflns_limit_l_max               12
_diffrn_reflns_reduction_process         ?

_diffrn_standards_number                 ?
_diffrn_standards_interval_count         ?
_diffrn_standards_interval_time          ?
_diffrn_standards_decay_%                ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
  ? ? ?

_diffrn_radiation_probe                  X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details
; ?
;

_reflns_number_total                     1626
_reflns_number_gt                        1024
_reflns_threshold_expression             'I>3σ(I)'

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_R_factor_gt                   0.0261
_refine_ls_wR_factor_gt                  0.0484
_refine_ls_R_factor_all                  0.0511
_refine_ls_wR_factor_ref                 0.0537
_refine_ls_goodness_of_fit_ref           1.09
_refine_ls_goodness_of_fit_gt            1.26
_refine_ls_restrained_S_gt               ?
_refine_ls_restrained_S_all              ?
_refine_ls_number_reflns                 1626
_refine_ls_number_parameters             79
_refine_ls_number_restraints             0
_refine_ls_number_constraints            0
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0004I²)'
_refine_ls_hydrogen_treatment            ?
_refine_ls_shift/su_max                  0.0005
_refine_ls_shift/su_mean                 0.0001
_refine_diff_density_max                 2.79
_refine_diff_density_min                 -2.08
_refine_ls_extinction_method
 'B-C type 1 Lorentzian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef               55(14)
_refine_ls_extinction_expression         ?
_refine_ls_abs_structure_details         ?
_refine_ls_abs_structure_Flack           ?
_refine_ls_abs_structure_Rogers          ?

loop_
 _atom_type_symbol
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 Al   0.0645  0.0514
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Ba  -0.3244  2.2819
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Pt  -1.7033  8.3905
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection               ?
_computing_cell_refinement               ?
_computing_data_reduction                ?
_computing_structure_solution            ?
_computing_structure_refinement          ?
_computing_molecular_graphics            ?
_computing_publication_material          ?

loop_
 _restr_distance_atom_site_label_1
 _restr_distance_site_symmetry_1
 _restr_distance_atom_site_label_2
 _restr_distance_site_symmetry_2
 _restr_distance_target
 _restr_distance_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_angle_atom_site_label_1
 _restr_angle_site_symmetry_1
 _restr_angle_atom_site_label_2
 _restr_angle_site_symmetry_2
 _restr_angle_atom_site_label_3
 _restr_angle_site_symmetry_3
 _restr_angle_target
 _restr_angle_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_torsion_atom_site_label_1
 _restr_torsion_site_symmetry_1
 _restr_torsion_atom_site_label_2
 _restr_torsion_site_symmetry_2
 _restr_torsion_atom_site_label_3
 _restr_torsion_site_symmetry_3
 _restr_torsion_atom_site_label_4
 _restr_torsion_site_symmetry_4
 _restr_torsion_angle_target
 _restr_torsion_weight_param
 ? ? ? ? ? ? ? ? ? ?

loop_
 _restr_equal_distance_atom_site_label_1
 _restr_equal_distance_site_symmetry_1
 _restr_equal_distance_atom_site_label_2
 _restr_equal_distance_site_symmetry_2
 _restr_equal_distance_class_class_id
 _restr_equal_distance_class_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_equal_angle_atom_site_label_1
 _restr_equal_angle_site_symmetry_1
 _restr_equal_angle_atom_site_label_2
 _restr_equal_angle_site_symmetry_2
 _restr_equal_angle_atom_site_label_3
 _restr_equal_angle_site_symmetry_3
 _restr_equal_angle_class_class_id
 _restr_equal_angle_class_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_equal_torsion_atom_site_label_1
 _restr_equal_torsion_site_symmetry_1
 _restr_equal_torsion_atom_site_label_2
 _restr_equal_torsion_site_symmetry_2
 _restr_equal_torsion_atom_site_label_3
 _restr_equal_torsion_site_symmetry_3
 _restr_equal_torsion_atom_site_label_4
 _restr_equal_torsion_site_symmetry_4
 _restr_equal_torsion_class_class_id
 _restr_equal_torsion_class_target_weight_param
 ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
  Ba Ba 0.25019(5) 0 0.06630(4) Uani 0.01545(19) 12 1 d . . .
  Pt1 Pt 0.50224(4) 0 0.14022(2) Uani 0.01444(11) 12 1 d . . .
  Pt2 Pt 0.16813(4) 0.33804(3) 0.25 Uani 0.01437(15) 12 1 d . . .
  Pt3 Pt 0.243527(17) 0.48705(3) 0 Uani 0.01417(11) 12 1 d . . .
  Pt4 Pt 0 0 0.14818(4) Uani 0.0153(2) 4 0.961(4) d . . .
  Pt5 Pt 0.333333 0.666667 0.25 Uani 0.01461(15) 4 1 d . . .
  Al1 Al 0.1763(2) 0.4919(2) 0.15558(16) Uani 0.0159(9) 24 1 d . . .
  Al2 Al 0.2863(2) 0.3927(2) 0.11052(15) Uani 0.0160(10) 24 1 d . . .
  Al3 Al 0.8136(3) 0 0.1636(2) Uani 0.0163(11) 12 1 d . . .
  Al4 Al 0.3680(3) 0.5028(3) 0.25 Uani 0.0164(13) 12 1 d . . .
  Al5 Al 0.55490(13) 0.1098(3) 0 Uani 0.0151(9) 12 1 d . . .
  Al6 Al 0.333333 0.666667 0.0834(2) Uani 0.0153(9) 8 1 d . . .
  Al7 Al 0.1444(4) 0 0.25 Uani 0.0156(16) 6 1 d . . .
  Al8 Al 0.3623(4) 0 0.25 Uani 0.0156(16) 6 1 d . . .
  Al9 Al 0 0 0 Uani 0.022(2) 2 1 d . . .


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_E_label
 _jana_atom_site_ADP_E_type_symbol
 _jana_atom_site_ADP_E_11111
 _jana_atom_site_ADP_E_11112
 _jana_atom_site_ADP_E_11113
 _jana_atom_site_ADP_E_11122
 _jana_atom_site_ADP_E_11123
 _jana_atom_site_ADP_E_11133
 _jana_atom_site_ADP_E_11222
 _jana_atom_site_ADP_E_11223
 _jana_atom_site_ADP_E_11233
 _jana_atom_site_ADP_E_11333
 _jana_atom_site_ADP_E_12222
 _jana_atom_site_ADP_E_12223
 _jana_atom_site_ADP_E_12233
 _jana_atom_site_ADP_E_12333
 _jana_atom_site_ADP_E_13333
 _jana_atom_site_ADP_E_22222
 _jana_atom_site_ADP_E_22223
 _jana_atom_site_ADP_E_22233
 _jana_atom_site_ADP_E_22333
 _jana_atom_site_ADP_E_23333
 _jana_atom_site_ADP_E_33333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_F_label
 _jana_atom_site_ADP_F_type_symbol
 _jana_atom_site_ADP_F_111111
 _jana_atom_site_ADP_F_111112
 _jana_atom_site_ADP_F_111113
 _jana_atom_site_ADP_F_111122
 _jana_atom_site_ADP_F_111123
 _jana_atom_site_ADP_F_111133
 _jana_atom_site_ADP_F_111222
 _jana_atom_site_ADP_F_111223
 _jana_atom_site_ADP_F_111233
 _jana_atom_site_ADP_F_111333
 _jana_atom_site_ADP_F_112222
 _jana_atom_site_ADP_F_112223
 _jana_atom_site_ADP_F_112233
 _jana_atom_site_ADP_F_112333
 _jana_atom_site_ADP_F_113333
 _jana_atom_site_ADP_F_122222
 _jana_atom_site_ADP_F_122223
 _jana_atom_site_ADP_F_122233
 _jana_atom_site_ADP_F_122333
 _jana_atom_site_ADP_F_123333
 _jana_atom_site_ADP_F_133333
 _jana_atom_site_ADP_F_222222
 _jana_atom_site_ADP_F_222223
 _jana_atom_site_ADP_F_222233
 _jana_atom_site_ADP_F_222333
 _jana_atom_site_ADP_F_223333
 _jana_atom_site_ADP_F_233333
 _jana_atom_site_ADP_F_333333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba Pt1 . . 3.7874(11) ?
  Ba Pt2 . 3_555 3.6189(7) ?
  Ba Pt2 . 7_555 3.6189(7) ?
  Ba Pt3 . 3_555 3.5897(8) ?
  Ba Pt3 . 14_555 3.5897(11) ?
  Ba Pt4 . . 3.8049(10) ?
  Ba Al1 . 3_555 3.408(4) ?
  Ba Al1 . 22_555 3.408(3) ?
  Ba Al2 . 3_555 3.607(3) ?
  Ba Al2 . 12_555 3.389(3) ?
  Ba Al2 . 14_555 3.389(3) ?
  Ba Al2 . 22_555 3.607(3) ?
  Ba Al3 . 2_545 3.574(2) ?
  Ba Al3 . 3_665 3.574(5) ?
  Ba Al3 . 11_655 3.818(4) ?
  Ba Al5 . . 3.959(2) ?
  Ba Al5 . 13_655 3.959(3) ?
  Ba Al7 . . 3.326(3) ?
  Ba Al8 . . 3.367(3) ?
  Ba Al9 . . 3.7251(10) ?
  Pt1 Pt1 . 8_555 3.5419(5) ?
  Pt1 Al1 . 3_555 2.604(3) ?
  Pt1 Al1 . 22_555 2.604(4) ?
  Pt1 Al2 . 2_655 2.656(5) ?
  Pt1 Al2 . 24_655 2.656(3) ?
  Pt1 Al4 . 2_655 2.589(5) ?
  Pt1 Al4 . 9_655 2.589(3) ?
  Pt1 Al5 . . 2.6376(18) ?
  Pt1 Al5 . 13_655 2.6376(17) ?
  Pt1 Al8 . . 2.668(4) ?
  Pt2 Al1 . . 2.625(3) ?
  Pt2 Al1 . 16_555 2.625(3) ?
  Pt2 Al2 . . 2.683(3) ?
  Pt2 Al2 . 16_555 2.683(3) ?
  Pt2 Al3 . 3_665 2.693(4) ?
  Pt2 Al3 . 9_665 2.693(4) ?
  Pt2 Al4 . . 2.636(4) ?
  Pt2 Al7 . 2_555 2.599(3) ?
  Pt2 Al8 . 2_555 2.588(4) ?
  Pt3 Pt3 . 2_665 3.8425(12) ?
  Pt3 Pt3 . 3_565 3.8425(10) ?
  Pt3 Al1 . . 2.700(3) ?
  Pt3 Al1 . 11_555 2.700(3) ?
  Pt3 Al2 . . 2.487(3) ?
  Pt3 Al2 . 11_555 2.487(3) ?
  Pt3 Al5 . 14_565 2.534(5) ?
  Pt3 Al5 . 15_555 2.534(4) ?
  Pt3 Al6 . . 2.594(2) ?
  Pt3 Al6 . 10_665 2.594(2) ?
  Pt4 Pt4 . 7_555 3.2849(10) ?
  Pt4 Al3 . 1_455 2.670(4) ?
  Pt4 Al3 . 2_545 2.670(4) ?
  Pt4 Al3 . 3_665 2.670(3) ?
  Pt4 Al7 . . 2.634(4) ?
  Pt4 Al7 . 2_555 2.634(4) ?
  Pt4 Al7 . 3_555 2.634(3) ?
  Pt4 Al9 . . 2.3904(7) ?
  Pt5 Al1 . . 2.822(2) ?
  Pt5 Al1 . 2_665 2.822(3) ?
  Pt5 Al1 . 3_565 2.822(4) ?
  Pt5 Al1 . 16_555 2.822(2) ?
  Pt5 Al1 . 17_665 2.822(3) ?
  Pt5 Al1 . 18_565 2.822(4) ?
  Pt5 Al4 . . 2.619(5) ?
  Pt5 Al4 . 2_665 2.619(5) ?
  Pt5 Al4 . 3_565 2.619(7) ?
  Pt5 Al6 . . 2.688(4) ?
  Pt5 Al6 . 16_555 2.688(4) ?
  Al1 Al1 . 16_555 3.046(4) ?
  Al1 Al2 . . 2.685(5) ?
  Al1 Al2 . 3_565 3.833(6) ?
  Al1 Al4 . . 3.064(6) ?
  Al1 Al4 . 3_565 2.801(6) ?
  Al1 Al5 . 14_565 2.976(4) ?
  Al1 Al6 . . 2.646(3) ?
  Al1 Al8 . 2_555 2.723(3) ?
  Al2 Al2 . 22_555 2.628(6) ?
  Al2 Al3 . 3_665 2.688(5) ?
  Al2 Al4 . . 2.656(3) ?
  Al2 Al4 . 7_555 3.976(6) ?
  Al2 Al5 . 3_665 3.943(5) ?
  Al2 Al5 . 15_555 2.902(3) ?
  Al2 Al6 . . 3.646(4) ?
  Al3 Al3 . 8_555 2.788(5) ?
  Al3 Al7 . 2_655 2.789(3) ?
  Al3 Al7 . 3_655 2.789(6) ?
  Al3 Al9 . 1_655 3.746(4) ?
  Al4 Al4 . 7_555 3.331(8) ?
  Al4 Al6 . . 3.753(5) ?
  Al4 Al6 . 16_555 3.753(5) ?
  Al4 Al8 . 3_665 3.332(7) ?
  Al5 Al5 . 13_655 2.713(5) ?
  Al5 Al6 . 13_665 3.071(3) ?
  Al5 Al6 . 22_555 3.071(3) ?
  Al6 Al6 . 10_665 2.690(5) ?
  Al7 Al7 . 2_555 3.566(7) ?
  Al7 Al7 . 3_555 3.566(7) ?
  Al7 Al8 . . 3.108(8) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  Pt1 Ba Pt2 . . 3_555 74.218(18) ?
  Pt1 Ba Pt2 . . 7_555 74.218(16) ?
  Pt1 Ba Pt3 . . 3_555 70.108(15) ?
  Pt1 Ba Pt3 . . 14_555 70.108(17) ?
  Pt1 Ba Pt4 . . . 141.33(2) ?
  Pt1 Ba Al1 . . 3_555 42.02(6) ?
  Pt1 Ba Al1 . . 22_555 42.02(6) ?
  Pt1 Ba Al2 . . 3_555 86.57(7) ?
  Pt1 Ba Al2 . . 12_555 84.74(6) ?
  Pt1 Ba Al2 . . 14_555 84.74(7) ?
  Pt1 Ba Al2 . . 22_555 86.57(6) ?
  Pt1 Ba Al3 . . 2_545 117.15(6) ?
  Pt1 Ba Al3 . . 3_665 117.15(6) ?
  Pt1 Ba Al3 . . 11_655 122.14(6) ?
  Pt1 Ba Al5 . . . 39.73(3) ?
  Pt1 Ba Al5 . . 13_655 39.733(17) ?
  Pt1 Ba Al7 . . . 98.64(9) ?
  Pt1 Ba Al8 . . . 43.30(9) ?
  Pt1 Ba Al9 . . . 178.33(2) ?
  Pt2 Ba Pt2 3_555 . 7_555 70.033(16) ?
  Pt2 Ba Pt3 3_555 . 3_555 75.896(13) ?
  Pt2 Ba Pt3 3_555 . 14_555 135.89(2) ?
  Pt2 Ba Pt4 3_555 . . 74.319(19) ?
  Pt2 Ba Al1 3_555 . 3_555 43.75(6) ?
  Pt2 Ba Al1 3_555 . 22_555 90.63(5) ?
  Pt2 Ba Al2 3_555 . 3_555 43.58(4) ?
  Pt2 Ba Al2 3_555 . 12_555 117.46(7) ?
  Pt2 Ba Al2 3_555 . 14_555 154.97(9) ?
  Pt2 Ba Al2 3_555 . 22_555 113.62(4) ?
  Pt2 Ba Al3 3_555 . 2_545 43.97(5) ?
  Pt2 Ba Al3 3_555 . 3_665 91.11(6) ?
  Pt2 Ba Al3 3_555 . 11_655 143.02(2) ?
  Pt2 Ba Al5 3_555 . . 113.85(4) ?
  Pt2 Ba Al5 3_555 . 13_655 90.64(3) ?
  Pt2 Ba Al7 3_555 . . 43.71(5) ?
  Pt2 Ba Al8 3_555 . . 43.30(5) ?
  Pt2 Ba Al9 3_555 . . 104.44(2) ?
  Pt2 Ba Pt3 7_555 . 3_555 135.89(2) ?
  Pt2 Ba Pt3 7_555 . 14_555 75.897(11) ?
  Pt2 Ba Pt4 7_555 . . 74.319(17) ?
  Pt2 Ba Al1 7_555 . 3_555 90.63(5) ?
  Pt2 Ba Al1 7_555 . 22_555 43.75(5) ?
  Pt2 Ba Al2 7_555 . 3_555 113.62(4) ?
  Pt2 Ba Al2 7_555 . 12_555 154.97(5) ?
  Pt2 Ba Al2 7_555 . 14_555 117.46(6) ?
  Pt2 Ba Al2 7_555 . 22_555 43.58(4) ?
  Pt2 Ba Al3 7_555 . 2_545 91.11(6) ?
  Pt2 Ba Al3 7_555 . 3_665 43.97(6) ?
  Pt2 Ba Al3 7_555 . 11_655 143.02(2) ?
  Pt2 Ba Al5 7_555 . . 90.64(3) ?
  Pt2 Ba Al5 7_555 . 13_655 113.85(3) ?
  Pt2 Ba Al7 7_555 . . 43.71(5) ?
  Pt2 Ba Al8 7_555 . . 43.30(5) ?
  Pt2 Ba Al9 7_555 . . 104.441(18) ?
  Pt3 Ba Pt3 3_555 . 14_555 113.84(2) ?
  Pt3 Ba Pt4 3_555 . . 122.160(14) ?
  Pt3 Ba Al1 3_555 . 3_555 45.29(5) ?
  Pt3 Ba Al1 3_555 . 22_555 111.57(7) ?
  Pt3 Ba Al2 3_555 . 3_555 40.42(6) ?
  Pt3 Ba Al2 3_555 . 12_555 41.62(7) ?
  Pt3 Ba Al2 3_555 . 14_555 84.39(8) ?
  Pt3 Ba Al2 3_555 . 22_555 151.82(6) ?
  Pt3 Ba Al3 3_555 . 2_545 82.97(6) ?
  Pt3 Ba Al3 3_555 . 3_665 163.13(5) ?
  Pt3 Ba Al3 3_555 . 11_655 79.61(3) ?
  Pt3 Ba Al5 3_555 . . 78.17(5) ?
  Pt3 Ba Al5 3_555 . 13_655 38.83(4) ?
  Pt3 Ba Al7 3_555 . . 118.23(3) ?
  Pt3 Ba Al8 3_555 . . 92.58(5) ?
  Pt3 Ba Al9 3_555 . . 110.641(15) ?
  Pt3 Ba Pt4 14_555 . . 122.160(16) ?
  Pt3 Ba Al1 14_555 . 3_555 111.57(6) ?
  Pt3 Ba Al1 14_555 . 22_555 45.29(5) ?
  Pt3 Ba Al2 14_555 . 3_555 151.82(8) ?
  Pt3 Ba Al2 14_555 . 12_555 84.39(5) ?
  Pt3 Ba Al2 14_555 . 14_555 41.62(5) ?
  Pt3 Ba Al2 14_555 . 22_555 40.42(5) ?
  Pt3 Ba Al3 14_555 . 2_545 163.13(7) ?
  Pt3 Ba Al3 14_555 . 3_665 82.97(5) ?
  Pt3 Ba Al3 14_555 . 11_655 79.61(3) ?
  Pt3 Ba Al5 14_555 . . 38.83(6) ?
  Pt3 Ba Al5 14_555 . 13_655 78.17(4) ?
  Pt3 Ba Al7 14_555 . . 118.23(3) ?
  Pt3 Ba Al8 14_555 . . 92.58(5) ?
  Pt3 Ba Al9 14_555 . . 110.641(17) ?
  Pt4 Ba Al1 . . 3_555 117.12(6) ?
  Pt4 Ba Al1 . . 22_555 117.12(6) ?
  Pt4 Ba Al2 . . 3_555 85.92(8) ?
  Pt4 Ba Al2 . . 12_555 130.14(6) ?
  Pt4 Ba Al2 . . 14_555 130.14(8) ?
  Pt4 Ba Al2 . . 22_555 85.92(6) ?
  Pt4 Ba Al3 . . 2_545 42.28(6) ?
  Pt4 Ba Al3 . . 3_665 42.28(5) ?
  Pt4 Ba Al3 . . 11_655 96.53(6) ?
  Pt4 Ba Al5 . . . 159.66(5) ?
  Pt4 Ba Al5 . . 13_655 159.66(4) ?
  Pt4 Ba Al7 . . . 42.69(8) ?
  Pt4 Ba Al8 . . . 98.03(9) ?
  Pt4 Ba Al9 . . . 36.999(13) ?
  Al1 Ba Al1 3_555 . 22_555 79.45(8) ?
  Al1 Ba Al2 3_555 . 3_555 44.89(9) ?
  Al1 Ba Al2 3_555 . 12_555 82.32(9) ?
  Al1 Ba Al2 3_555 . 14_555 111.23(10) ?
  Al1 Ba Al2 3_555 . 22_555 123.00(7) ?
  Al1 Ba Al3 3_555 . 2_545 78.77(8) ?
  Al1 Ba Al3 3_555 . 3_665 128.95(8) ?
  Al1 Ba Al3 3_555 . 11_655 124.30(6) ?
  Al1 Ba Al5 3_555 . . 75.81(8) ?
  Al1 Ba Al5 3_555 . 13_655 46.92(7) ?
  Al1 Ba Al7 3_555 . . 85.13(9) ?
  Al1 Ba Al8 3_555 . . 47.39(6) ?
  Al1 Ba Al9 3_555 . . 137.47(6) ?
  Al1 Ba Al2 22_555 . 3_555 123.00(9) ?
  Al1 Ba Al2 22_555 . 12_555 111.23(7) ?
  Al1 Ba Al2 22_555 . 14_555 82.32(6) ?
  Al1 Ba Al2 22_555 . 22_555 44.89(9) ?
  Al1 Ba Al3 22_555 . 2_545 128.95(7) ?
  Al1 Ba Al3 22_555 . 3_665 78.77(8) ?
  Al1 Ba Al3 22_555 . 11_655 124.30(6) ?
  Al1 Ba Al5 22_555 . . 46.92(6) ?
  Al1 Ba Al5 22_555 . 13_655 75.81(7) ?
  Al1 Ba Al7 22_555 . . 85.13(8) ?
  Al1 Ba Al8 22_555 . . 47.39(6) ?
  Al1 Ba Al9 22_555 . . 137.47(7) ?
  Al2 Ba Al2 3_555 . 12_555 77.72(8) ?
  Al2 Ba Al2 3_555 . 14_555 123.20(9) ?
  Al2 Ba Al2 3_555 . 22_555 157.19(6) ?
  Al2 Ba Al3 3_555 . 2_545 43.96(10) ?
  Al2 Ba Al3 3_555 . 3_665 122.88(8) ?
  Al2 Ba Al3 3_555 . 11_655 101.04(4) ?
  Al2 Ba Al5 3_555 . . 113.05(10) ?
  Al2 Ba Al5 3_555 . 13_655 73.74(8) ?
  Al2 Ba Al7 3_555 . . 79.78(5) ?
  Al2 Ba Al8 3_555 . . 80.05(5) ?
  Al2 Ba Al9 3_555 . . 93.11(8) ?
  Al2 Ba Al2 12_555 . 14_555 45.63(9) ?
  Al2 Ba Al2 12_555 . 22_555 123.20(7) ?
  Al2 Ba Al3 12_555 . 2_545 110.80(8) ?
  Al2 Ba Al3 12_555 . 3_665 148.72(10) ?
  Al2 Ba Al3 12_555 . 11_655 43.29(9) ?
  Al2 Ba Al5 12_555 . . 64.36(5) ?
  Al2 Ba Al5 12_555 . 13_655 45.71(7) ?
  Al2 Ba Al7 12_555 . . 157.01(6) ?
  Al2 Ba Al8 12_555 . . 124.22(11) ?
  Al2 Ba Al9 12_555 . . 96.79(6) ?
  Al2 Ba Al2 14_555 . 22_555 77.72(8) ?
  Al2 Ba Al3 14_555 . 2_545 148.72(7) ?
  Al2 Ba Al3 14_555 . 3_665 110.80(10) ?
  Al2 Ba Al3 14_555 . 11_655 43.29(7) ?
  Al2 Ba Al5 14_555 . . 45.71(6) ?
  Al2 Ba Al5 14_555 . 13_655 64.36(9) ?
  Al2 Ba Al7 14_555 . . 157.01(8) ?
  Al2 Ba Al8 14_555 . . 124.22(10) ?
  Al2 Ba Al9 14_555 . . 96.79(7) ?
  Al2 Ba Al3 22_555 . 2_545 122.88(8) ?
  Al2 Ba Al3 22_555 . 3_665 43.96(7) ?
  Al2 Ba Al3 22_555 . 11_655 101.04(4) ?
  Al2 Ba Al5 22_555 . . 73.74(8) ?
  Al2 Ba Al5 22_555 . 13_655 113.05(7) ?
  Al2 Ba Al7 22_555 . . 79.78(4) ?
  Al2 Ba Al8 22_555 . . 80.05(5) ?
  Al2 Ba Al9 22_555 . . 93.11(6) ?
  Al3 Ba Al3 2_545 . 3_665 80.20(8) ?
  Al3 Ba Al3 2_545 . 11_655 106.09(7) ?
  Al3 Ba Al5 2_545 . . 154.54(8) ?
  Al3 Ba Al5 2_545 . 13_655 117.49(7) ?
  Al3 Ba Al7 2_545 . . 47.51(7) ?
  Al3 Ba Al8 2_545 . . 84.89(9) ?
  Al3 Ba Al9 2_545 . . 61.71(6) ?
  Al3 Ba Al3 3_665 . 11_655 106.09(8) ?
  Al3 Ba Al5 3_665 . . 117.49(7) ?
  Al3 Ba Al5 3_665 . 13_655 154.54(6) ?
  Al3 Ba Al7 3_665 . . 47.51(7) ?
  Al3 Ba Al8 3_665 . . 84.89(9) ?
  Al3 Ba Al9 3_665 . . 61.71(6) ?
  Al3 Ba Al5 11_655 . . 87.25(6) ?
  Al3 Ba Al5 11_655 . 13_655 87.25(6) ?
  Al3 Ba Al7 11_655 . . 139.22(11) ?
  Al3 Ba Al8 11_655 . . 165.44(11) ?
  Al3 Ba Al9 11_655 . . 59.53(6) ?
  Al5 Ba Al5 . . 13_655 40.06(7) ?
  Al5 Ba Al7 . . . 130.47(8) ?
  Al5 Ba Al8 . . . 79.08(8) ?
  Al5 Ba Al9 . . . 141.67(4) ?
  Al5 Ba Al7 13_655 . . 130.47(8) ?
  Al5 Ba Al8 13_655 . . 79.08(8) ?
  Al5 Ba Al9 13_655 . . 141.67(2) ?
  Al7 Ba Al8 . . . 55.34(12) ?
  Al7 Ba Al9 . . . 79.69(9) ?
  Al8 Ba Al9 . . . 135.03(9) ?
  Ba Pt1 Pt1 . . 8_555 108.351(18) ?
  Ba Pt1 Al1 . . 3_555 61.17(10) ?
  Ba Pt1 Al1 . . 22_555 61.17(6) ?
  Ba Pt1 Al2 . . 2_655 138.59(6) ?
  Ba Pt1 Al2 . . 24_655 138.59(9) ?
  Ba Pt1 Al4 . . 2_655 122.79(9) ?
  Ba Pt1 Al4 . . 9_655 122.79(15) ?
  Ba Pt1 Al5 . . . 73.65(5) ?
  Ba Pt1 Al5 . . 13_655 73.65(7) ?
  Ba Pt1 Al8 . . . 59.93(8) ?
  Pt1 Pt1 Al1 8_555 . 3_555 84.54(6) ?
  Pt1 Pt1 Al1 8_555 . 22_555 84.54(6) ?
  Pt1 Pt1 Al2 8_555 . 2_655 100.39(6) ?
  Pt1 Pt1 Al2 8_555 . 24_655 100.39(5) ?
  Pt1 Pt1 Al4 8_555 . 2_655 46.83(10) ?
  Pt1 Pt1 Al4 8_555 . 9_655 46.83(6) ?
  Pt1 Pt1 Al5 8_555 . . 149.05(6) ?
  Pt1 Pt1 Al5 8_555 . 13_655 149.05(6) ?
  Pt1 Pt1 Al8 8_555 . . 48.42(8) ?
  Al1 Pt1 Al1 3_555 . 22_555 113.55(12) ?
  Al1 Pt1 Al2 3_555 . 2_655 93.55(12) ?
  Al1 Pt1 Al2 3_555 . 24_655 152.85(15) ?
  Al1 Pt1 Al4 3_555 . 2_655 65.30(12) ?
  Al1 Pt1 Al4 3_555 . 9_655 131.19(8) ?
  Al1 Pt1 Al5 3_555 . . 120.35(8) ?
  Al1 Pt1 Al5 3_555 . 13_655 69.20(7) ?
  Al1 Pt1 Al8 3_555 . . 62.17(9) ?
  Al1 Pt1 Al2 22_555 . 2_655 152.85(9) ?
  Al1 Pt1 Al2 22_555 . 24_655 93.55(12) ?
  Al1 Pt1 Al4 22_555 . 2_655 131.19(12) ?
  Al1 Pt1 Al4 22_555 . 9_655 65.30(17) ?
  Al1 Pt1 Al5 22_555 . . 69.20(10) ?
  Al1 Pt1 Al5 22_555 . 13_655 120.35(10) ?
  Al1 Pt1 Al8 22_555 . . 62.17(6) ?
  Al2 Pt1 Al2 2_655 . 24_655 59.32(12) ?
  Al2 Pt1 Al4 2_655 . 2_655 60.85(13) ?
  Al2 Pt1 Al4 2_655 . 9_655 98.60(16) ?
  Al2 Pt1 Al5 2_655 . . 96.32(10) ?
  Al2 Pt1 Al5 2_655 . 13_655 66.49(9) ?
  Al2 Pt1 Al8 2_655 . . 139.08(8) ?
  Al2 Pt1 Al4 24_655 . 2_655 98.60(13) ?
  Al2 Pt1 Al4 24_655 . 9_655 60.85(11) ?
  Al2 Pt1 Al5 24_655 . . 66.49(8) ?
  Al2 Pt1 Al5 24_655 . 13_655 96.32(7) ?
  Al2 Pt1 Al8 24_655 . . 139.08(9) ?
  Al4 Pt1 Al4 2_655 . 9_655 80.08(15) ?
  Al4 Pt1 Al5 2_655 . . 157.17(14) ?
  Al4 Pt1 Al5 2_655 . 13_655 105.07(12) ?
  Al4 Pt1 Al8 2_655 . . 78.64(13) ?
  Al4 Pt1 Al5 9_655 . . 105.07(10) ?
  Al4 Pt1 Al5 9_655 . 13_655 157.17(10) ?
  Al4 Pt1 Al8 9_655 . . 78.64(12) ?
  Al5 Pt1 Al5 . . 13_655 61.89(9) ?
  Al5 Pt1 Al8 . . . 124.06(10) ?
  Al5 Pt1 Al8 13_655 . . 124.06(8) ?
  Ba Pt2 Ba 2_555 . 7_555 109.940(17) ?
  Ba Pt2 Al1 2_555 . . 63.85(5) ?
  Ba Pt2 Al1 2_555 . 16_555 120.62(8) ?
  Ba Pt2 Al2 2_555 . . 67.98(6) ?
  Ba Pt2 Al2 2_555 . 16_555 176.98(6) ?
  Ba Pt2 Al3 2_555 . 3_665 67.14(9) ?
  Ba Pt2 Al3 2_555 . 9_665 117.34(7) ?
  Ba Pt2 Al4 2_555 . . 122.86(3) ?
  Ba Pt2 Al7 2_555 . 2_555 62.13(4) ?
  Ba Pt2 Al8 2_555 . 2_555 63.16(4) ?
  Ba Pt2 Al1 7_555 . . 120.62(8) ?
  Ba Pt2 Al1 7_555 . 16_555 63.85(5) ?
  Ba Pt2 Al2 7_555 . . 176.98(6) ?
  Ba Pt2 Al2 7_555 . 16_555 67.98(6) ?
  Ba Pt2 Al3 7_555 . 3_665 117.34(7) ?
  Ba Pt2 Al3 7_555 . 9_665 67.14(9) ?
  Ba Pt2 Al4 7_555 . . 122.86(3) ?
  Ba Pt2 Al7 7_555 . 2_555 62.13(4) ?
  Ba Pt2 Al8 7_555 . 2_555 63.16(4) ?
  Al1 Pt2 Al1 . . 16_555 70.93(9) ?
  Al1 Pt2 Al2 . . . 60.76(11) ?
  Al1 Pt2 Al2 . . 16_555 119.00(9) ?
  Al1 Pt2 Al3 . . 3_665 112.90(11) ?
  Al1 Pt2 Al3 . . 9_665 171.82(11) ?
  Al1 Pt2 Al4 . . . 71.24(11) ?
  Al1 Pt2 Al7 . . 2_555 121.34(9) ?
  Al1 Pt2 Al8 . . 2_555 62.96(11) ?
  Al1 Pt2 Al2 16_555 . . 119.00(9) ?
  Al1 Pt2 Al2 16_555 . 16_555 60.76(11) ?
  Al1 Pt2 Al3 16_555 . 3_665 171.82(11) ?
  Al1 Pt2 Al3 16_555 . 9_665 112.90(11) ?
  Al1 Pt2 Al4 16_555 . . 71.24(11) ?
  Al1 Pt2 Al7 16_555 . 2_555 121.34(9) ?
  Al1 Pt2 Al8 16_555 . 2_555 62.96(11) ?
  Al2 Pt2 Al2 . . 16_555 114.02(8) ?
  Al2 Pt2 Al3 . . 3_665 60.01(10) ?
  Al2 Pt2 Al3 . . 9_665 111.62(12) ?
  Al2 Pt2 Al4 . . . 59.92(6) ?
  Al2 Pt2 Al7 . . 2_555 114.86(7) ?
  Al2 Pt2 Al8 . . 2_555 116.78(9) ?
  Al2 Pt2 Al3 16_555 . 3_665 111.62(12) ?
  Al2 Pt2 Al3 16_555 . 9_665 60.01(10) ?
  Al2 Pt2 Al4 16_555 . . 59.92(6) ?
  Al2 Pt2 Al7 16_555 . 2_555 114.86(7) ?
  Al2 Pt2 Al8 16_555 . 2_555 116.78(9) ?
  Al3 Pt2 Al3 3_665 . 9_665 62.35(12) ?
  Al3 Pt2 Al4 3_665 . . 102.72(12) ?
  Al3 Pt2 Al7 3_665 . 2_555 63.57(10) ?
  Al3 Pt2 Al8 3_665 . 2_555 125.13(11) ?
  Al3 Pt2 Al4 9_665 . . 102.72(12) ?
  Al3 Pt2 Al7 9_665 . 2_555 63.57(10) ?
  Al3 Pt2 Al8 9_665 . 2_555 125.13(11) ?
  Al4 Pt2 Al7 . . 2_555 163.56(16) ?
  Al4 Pt2 Al8 . . 2_555 122.82(16) ?
  Al7 Pt2 Al8 2_555 . 2_555 73.62(14) ?
  Ba Pt3 Ba 2_555 . 12_555 70.826(18) ?
  Ba Pt3 Pt3 2_555 . 2_665 162.614(10) ?
  Ba Pt3 Pt3 2_555 . 3_565 117.213(17) ?
  Ba Pt3 Al1 2_555 . . 63.79(5) ?
  Ba Pt3 Al1 2_555 . 11_555 118.54(6) ?
  Ba Pt3 Al2 2_555 . . 70.17(6) ?
  Ba Pt3 Al2 2_555 . 11_555 64.86(6) ?
  Ba Pt3 Al5 2_555 . 14_565 78.49(7) ?
  Ba Pt3 Al5 2_555 . 15_555 137.61(5) ?
  Ba Pt3 Al6 2_555 . . 122.85(6) ?
  Ba Pt3 Al6 2_555 . 10_665 148.36(3) ?
  Ba Pt3 Pt3 12_555 . 2_665 117.213(17) ?
  Ba Pt3 Pt3 12_555 . 3_565 162.614(11) ?
  Ba Pt3 Al1 12_555 . . 118.54(7) ?
  Ba Pt3 Al1 12_555 . 11_555 63.79(8) ?
  Ba Pt3 Al2 12_555 . . 64.86(7) ?
  Ba Pt3 Al2 12_555 . 11_555 70.17(11) ?
  Ba Pt3 Al5 12_555 . 14_565 137.61(6) ?
  Ba Pt3 Al5 12_555 . 15_555 78.50(5) ?
  Ba Pt3 Al6 12_555 . . 148.36(3) ?
  Ba Pt3 Al6 12_555 . 10_665 122.85(6) ?
  Pt3 Pt3 Pt3 2_665 . 3_565 60.000(15) ?
  Pt3 Pt3 Al1 2_665 . . 99.48(5) ?
  Pt3 Pt3 Al1 2_665 . 11_555 78.28(6) ?
  Pt3 Pt3 Al2 2_665 . . 98.51(5) ?
  Pt3 Pt3 Al2 2_665 . 11_555 131.60(6) ?
  Pt3 Pt3 Al5 2_665 . 14_565 100.68(7) ?
  Pt3 Pt3 Al5 2_665 . 15_555 40.68(5) ?
  Pt3 Pt3 Al6 2_665 . . 42.22(5) ?
  Pt3 Pt3 Al6 2_665 . 10_665 42.22(5) ?
  Pt3 Pt3 Al1 3_565 . . 78.28(7) ?
  Pt3 Pt3 Al1 3_565 . 11_555 99.48(8) ?
  Pt3 Pt3 Al2 3_565 . . 131.60(7) ?
  Pt3 Pt3 Al2 3_565 . 11_555 98.51(10) ?
  Pt3 Pt3 Al5 3_565 . 14_565 40.68(7) ?
  Pt3 Pt3 Al5 3_565 . 15_555 100.68(5) ?
  Pt3 Pt3 Al6 3_565 . . 42.22(5) ?
  Pt3 Pt3 Al6 3_565 . 10_665 42.22(5) ?
  Al1 Pt3 Al1 . . 11_555 177.46(8) ?
  Al1 Pt3 Al2 . . . 62.20(11) ?
  Al1 Pt3 Al2 . . 11_555 119.16(10) ?
  Al1 Pt3 Al5 . . 14_565 69.24(8) ?
  Al1 Pt3 Al5 . . 15_555 109.86(6) ?
  Al1 Pt3 Al6 . . . 59.94(8) ?
  Al1 Pt3 Al6 . . 10_665 117.58(9) ?
  Al1 Pt3 Al2 11_555 . . 119.16(12) ?
  Al1 Pt3 Al2 11_555 . 11_555 62.20(11) ?
  Al1 Pt3 Al5 11_555 . 14_565 109.86(10) ?
  Al1 Pt3 Al5 11_555 . 15_555 69.24(9) ?
  Al1 Pt3 Al6 11_555 . . 117.58(8) ?
  Al1 Pt3 Al6 11_555 . 10_665 59.94(9) ?
  Al2 Pt3 Al2 . . 11_555 124.09(10) ?
  Al2 Pt3 Al5 . . 14_565 129.94(8) ?
  Al2 Pt3 Al5 . . 15_555 70.62(7) ?
  Al2 Pt3 Al6 . . . 91.67(9) ?
  Al2 Pt3 Al6 . . 10_665 140.59(7) ?
  Al2 Pt3 Al5 11_555 . 14_565 70.62(12) ?
  Al2 Pt3 Al5 11_555 . 15_555 129.94(10) ?
  Al2 Pt3 Al6 11_555 . . 140.59(11) ?
  Al2 Pt3 Al6 11_555 . 10_665 91.67(9) ?
  Al5 Pt3 Al5 14_565 . 15_555 141.37(9) ?
  Al5 Pt3 Al6 14_565 . . 73.57(6) ?
  Al5 Pt3 Al6 14_565 . 10_665 73.57(6) ?
  Al5 Pt3 Al6 15_555 . . 73.57(5) ?
  Al5 Pt3 Al6 15_555 . 10_665 73.57(5) ?
  Al6 Pt3 Al6 . . 10_665 62.45(10) ?
  Ba Pt4 Ba . . 2_555 108.615(13) ?
  Ba Pt4 Ba . . 3_555 108.615(19) ?
  Ba Pt4 Pt4 . . 7_555 110.314(14) ?
  Ba Pt4 Al3 . . 1_455 165.02(9) ?
  Ba Pt4 Al3 . . 2_545 64.24(4) ?
  Ba Pt4 Al3 . . 3_665 64.24(10) ?
  Ba Pt4 Al7 . . . 58.90(7) ?
  Ba Pt4 Al7 . . 2_555 125.666(10) ?
  Ba Pt4 Al7 . . 3_555 125.67(15) ?
  Ba Pt4 Al9 . . . 69.686(14) ?
  Ba Pt4 Ba 2_555 . 3_555 108.615(19) ?
  Ba Pt4 Pt4 2_555 . 7_555 110.314(14) ?
  Ba Pt4 Al3 2_555 . 1_455 64.24(4) ?
  Ba Pt4 Al3 2_555 . 2_545 165.02(9) ?
  Ba Pt4 Al3 2_555 . 3_665 64.24(10) ?
  Ba Pt4 Al7 2_555 . . 125.666(10) ?
  Ba Pt4 Al7 2_555 . 2_555 58.90(7) ?
  Ba Pt4 Al7 2_555 . 3_555 125.67(15) ?
  Ba Pt4 Al9 2_555 . . 69.686(14) ?
  Ba Pt4 Pt4 3_555 . 7_555 110.314(14) ?
  Ba Pt4 Al3 3_555 . 1_455 64.24(4) ?
  Ba Pt4 Al3 3_555 . 2_545 64.24(4) ?
  Ba Pt4 Al3 3_555 . 3_665 165.02(9) ?
  Ba Pt4 Al7 3_555 . . 125.666(15) ?
  Ba Pt4 Al7 3_555 . 2_555 125.666(15) ?
  Ba Pt4 Al7 3_555 . 3_555 58.90(5) ?
  Ba Pt4 Al9 3_555 . . 69.686(14) ?
  Pt4 Pt4 Al3 7_555 . 1_455 84.66(8) ?
  Pt4 Pt4 Al3 7_555 . 2_545 84.66(8) ?
  Pt4 Pt4 Al3 7_555 . 3_665 84.66(8) ?
  Pt4 Pt4 Al7 7_555 . . 51.42(7) ?
  Pt4 Pt4 Al7 7_555 . 2_555 51.42(7) ?
  Pt4 Pt4 Al7 7_555 . 3_555 51.42(5) ?
  Pt4 Pt4 Al9 7_555 . . 180 ?
  Al3 Pt4 Al3 1_455 . 2_545 119.14(2) ?
  Al3 Pt4 Al3 1_455 . 3_665 119.14(11) ?
  Al3 Pt4 Al7 1_455 . . 136.08(11) ?
  Al3 Pt4 Al7 1_455 . 2_555 63.44(6) ?
  Al3 Pt4 Al7 1_455 . 3_555 63.44(15) ?
  Al3 Pt4 Al9 1_455 . . 95.34(8) ?
  Al3 Pt4 Al3 2_545 . 3_665 119.14(11) ?
  Al3 Pt4 Al7 2_545 . . 63.44(6) ?
  Al3 Pt4 Al7 2_545 . 2_555 136.08(11) ?
  Al3 Pt4 Al7 2_545 . 3_555 63.44(15) ?
  Al3 Pt4 Al9 2_545 . . 95.34(8) ?
  Al3 Pt4 Al7 3_665 . . 63.44(10) ?
  Al3 Pt4 Al7 3_665 . 2_555 63.44(10) ?
  Al3 Pt4 Al7 3_665 . 3_555 136.08(10) ?
  Al3 Pt4 Al9 3_665 . . 95.34(8) ?
  Al7 Pt4 Al7 . . 2_555 85.22(8) ?
  Al7 Pt4 Al7 . . 3_555 85.22(12) ?
  Al7 Pt4 Al9 . . . 128.58(7) ?
  Al7 Pt4 Al7 2_555 . 3_555 85.22(12) ?
  Al7 Pt4 Al9 2_555 . . 128.58(7) ?
  Al7 Pt4 Al9 3_555 . . 128.58(5) ?
  Al1 Pt5 Al1 . . 2_665 93.62(9) ?
  Al1 Pt5 Al1 . . 3_565 93.62(9) ?
  Al1 Pt5 Al1 . . 16_555 65.32(7) ?
  Al1 Pt5 Al1 . . 17_665 130.21(12) ?
  Al1 Pt5 Al1 . . 18_565 130.21(11) ?
  Al1 Pt5 Al4 . . . 68.42(10) ?
  Al1 Pt5 Al4 . . 2_665 147.11(5) ?
  Al1 Pt5 Al4 . . 3_565 61.84(11) ?
  Al1 Pt5 Al6 . . . 57.34(5) ?
  Al1 Pt5 Al6 . . 16_555 122.66(5) ?
  Al1 Pt5 Al1 2_665 . 3_565 93.62(12) ?
  Al1 Pt5 Al1 2_665 . 16_555 130.21(12) ?
  Al1 Pt5 Al1 2_665 . 17_665 65.32(9) ?
  Al1 Pt5 Al1 2_665 . 18_565 130.21(10) ?
  Al1 Pt5 Al4 2_665 . . 61.84(11) ?
  Al1 Pt5 Al4 2_665 . 2_665 68.42(14) ?
  Al1 Pt5 Al4 2_665 . 3_565 147.11(6) ?
  Al1 Pt5 Al6 2_665 . . 57.34(6) ?
  Al1 Pt5 Al6 2_665 . 16_555 122.66(6) ?
  Al1 Pt5 Al1 3_565 . 16_555 130.21(11) ?
  Al1 Pt5 Al1 3_565 . 17_665 130.21(10) ?
  Al1 Pt5 Al1 3_565 . 18_565 65.32(9) ?
  Al1 Pt5 Al4 3_565 . . 147.11(7) ?
  Al1 Pt5 Al4 3_565 . 2_665 61.84(13) ?
  Al1 Pt5 Al4 3_565 . 3_565 68.42(11) ?
  Al1 Pt5 Al6 3_565 . . 57.34(6) ?
  Al1 Pt5 Al6 3_565 . 16_555 122.66(6) ?
  Al1 Pt5 Al1 16_555 . 17_665 93.62(9) ?
  Al1 Pt5 Al1 16_555 . 18_565 93.62(9) ?
  Al1 Pt5 Al4 16_555 . . 68.42(10) ?
  Al1 Pt5 Al4 16_555 . 2_665 147.11(5) ?
  Al1 Pt5 Al4 16_555 . 3_565 61.84(11) ?
  Al1 Pt5 Al6 16_555 . . 122.66(5) ?
  Al1 Pt5 Al6 16_555 . 16_555 57.34(5) ?
  Al1 Pt5 Al1 17_665 . 18_565 93.62(12) ?
  Al1 Pt5 Al4 17_665 . . 61.84(11) ?
  Al1 Pt5 Al4 17_665 . 2_665 68.42(14) ?
  Al1 Pt5 Al4 17_665 . 3_565 147.11(6) ?
  Al1 Pt5 Al6 17_665 . . 122.66(6) ?
  Al1 Pt5 Al6 17_665 . 16_555 57.34(6) ?
  Al1 Pt5 Al4 18_565 . . 147.11(7) ?
  Al1 Pt5 Al4 18_565 . 2_665 61.84(13) ?
  Al1 Pt5 Al4 18_565 . 3_565 68.42(11) ?
  Al1 Pt5 Al6 18_565 . . 122.66(6) ?
  Al1 Pt5 Al6 18_565 . 16_555 57.34(6) ?
  Al4 Pt5 Al4 . . 2_665 120.00(17) ?
  Al4 Pt5 Al4 . . 3_565 120.00(13) ?
  Al4 Pt5 Al6 . . . 90 ?
  Al4 Pt5 Al6 . . 16_555 90 ?
  Al4 Pt5 Al4 2_665 . 3_565 120.00(18) ?
  Al4 Pt5 Al6 2_665 . . 90 ?
  Al4 Pt5 Al6 2_665 . 16_555 90 ?
  Al4 Pt5 Al6 3_565 . . 90 ?
  Al4 Pt5 Al6 3_565 . 16_555 90 ?
  Al6 Pt5 Al6 . . 16_555 180 ?
  Ba Al1 Pt1 2_555 . 2_555 76.81(6) ?
  Ba Al1 Pt2 2_555 . . 72.41(6) ?
  Ba Al1 Pt3 2_555 . . 70.92(6) ?
  Ba Al1 Pt5 2_555 . . 168.47(13) ?
  Ba Al1 Al1 2_555 . 16_555 115.00(9) ?
  Ba Al1 Al2 2_555 . . 71.49(8) ?
  Ba Al1 Al2 2_555 . 3_565 112.94(10) ?
  Ba Al1 Al4 2_555 . . 116.73(14) ?
  Ba Al1 Al4 2_555 . 3_565 129.73(15) ?
  Ba Al1 Al5 2_555 . 14_565 76.33(9) ?
  Ba Al1 Al6 2_555 . . 128.00(12) ?
  Ba Al1 Al8 2_555 . 2_555 65.52(9) ?
  Pt1 Al1 Pt2 2_555 . . 117.51(9) ?
  Pt1 Al1 Pt3 2_555 . . 106.16(10) ?
  Pt1 Al1 Pt5 2_555 . . 111.32(12) ?
  Pt1 Al1 Al1 2_555 . 16_555 95.46(12) ?
  Pt1 Al1 Al2 2_555 . . 147.07(11) ?
  Pt1 Al1 Al2 2_555 . 3_565 43.76(8) ?
  Pt1 Al1 Al4 2_555 . . 155.06(13) ?
  Pt1 Al1 Al4 2_555 . 3_565 57.09(13) ?
  Pt1 Al1 Al5 2_555 . 14_565 55.94(10) ?
  Pt1 Al1 Al6 2_555 . . 106.92(12) ?
  Pt1 Al1 Al8 2_555 . 2_555 60.08(11) ?
  Pt2 Al1 Pt3 . . . 112.71(13) ?
  Pt2 Al1 Pt5 . . . 96.27(9) ?
  Pt2 Al1 Al1 . . 16_555 54.54(8) ?
  Pt2 Al1 Al2 . . . 60.68(10) ?
  Pt2 Al1 Al2 . . 3_565 151.50(12) ?
  Pt2 Al1 Al4 . . . 54.54(9) ?
  Pt2 Al1 Al4 . . 3_565 110.11(11) ?
  Pt2 Al1 Al5 . . 14_565 148.63(12) ?
  Pt2 Al1 Al6 . . . 134.90(14) ?
  Pt2 Al1 Al8 . . 2_555 57.85(11) ?
  Pt3 Al1 Pt5 . . . 112.91(8) ?
  Pt3 Al1 Al1 . . 16_555 158.38(16) ?
  Pt3 Al1 Al2 . . . 55.00(9) ?
  Pt3 Al1 Al2 . . 3_565 94.99(9) ?
  Pt3 Al1 Al4 . . . 98.30(12) ?
  Pt3 Al1 Al4 . . 3_565 136.72(13) ?
  Pt3 Al1 Al5 . . 14_565 52.75(9) ?
  Pt3 Al1 Al6 . . . 58.05(8) ?
  Pt3 Al1 Al8 . . 2_555 136.21(11) ?
  Pt5 Al1 Al1 . . 16_555 57.34(6) ?
  Pt5 Al1 Al2 . . . 101.37(11) ?
  Pt5 Al1 Al2 . . 3_565 78.01(9) ?
  Pt5 Al1 Al4 . . . 52.65(9) ?
  Pt5 Al1 Al4 . . 3_565 55.51(12) ?
  Pt5 Al1 Al5 . . 14_565 114.85(11) ?
  Pt5 Al1 Al6 . . . 58.78(8) ?
  Pt5 Al1 Al8 . . 2_555 110.69(11) ?
  Al1 Al1 Al2 16_555 . . 105.71(14) ?
  Al1 Al1 Al2 16_555 . 3_565 100.93(12) ?
  Al1 Al1 Al4 16_555 . . 60.19(10) ?
  Al1 Al1 Al4 16_555 . 3_565 57.07(11) ?
  Al1 Al1 Al5 16_555 . 14_565 147.48(18) ?
  Al1 Al1 Al6 16_555 . . 116.12(12) ?
  Al1 Al1 Al8 16_555 . 2_555 55.98(7) ?
  Al2 Al1 Al2 . . 3_565 147.71(11) ?
  Al2 Al1 Al4 . . . 54.56(11) ?
  Al2 Al1 Al4 . . 3_565 155.60(16) ?
  Al2 Al1 Al5 . . 14_565 106.81(13) ?
  Al2 Al1 Al6 . . . 86.28(11) ?
  Al2 Al1 Al8 . . 2_555 112.22(17) ?
  Al2 Al1 Al4 3_565 . . 130.25(12) ?
  Al2 Al1 Al4 3_565 . 3_565 43.87(10) ?
  Al2 Al1 Al5 3_565 . 14_565 48.47(10) ?
  Al2 Al1 Al6 3_565 . . 65.53(9) ?
  Al2 Al1 Al8 3_565 . 2_555 97.66(16) ?
  Al4 Al1 Al4 . . 3_565 101.23(15) ?
  Al4 Al1 Al5 . . 14_565 144.56(12) ?
  Al4 Al1 Al6 . . . 81.83(10) ?
  Al4 Al1 Al8 . . 2_555 104.71(12) ?
  Al4 Al1 Al5 3_565 . 14_565 91.72(16) ?
  Al4 Al1 Al6 3_565 . . 87.04(12) ?
  Al4 Al1 Al8 3_565 . 2_555 74.18(16) ?
  Al5 Al1 Al6 14_565 . . 65.91(10) ?
  Al5 Al1 Al8 14_565 . 2_555 110.55(13) ?
  Al6 Al1 Al8 . . 2_555 160.9(2) ?
  Ba Al2 Ba 2_555 . 12_555 72.90(5) ?
  Ba Al2 Pt1 2_555 . 3_665 178.99(9) ?
  Ba Al2 Pt2 2_555 . . 68.44(6) ?
  Ba Al2 Pt3 2_555 . . 69.41(7) ?
  Ba Al2 Al1 2_555 . . 63.62(8) ?
  Ba Al2 Al1 2_555 . 2_665 137.44(13) ?
  Ba Al2 Al2 2_555 . 22_555 119.50(10) ?
  Ba Al2 Al3 2_555 . 3_665 67.37(10) ?
  Ba Al2 Al4 2_555 . . 122.60(14) ?
  Ba Al2 Al4 2_555 . 7_555 140.57(9) ?
  Ba Al2 Al5 2_555 . 3_665 137.40(8) ?
  Ba Al2 Al5 2_555 . 15_555 122.69(11) ?
  Ba Al2 Al6 2_555 . . 97.47(9) ?
  Ba Al2 Pt1 12_555 . 3_665 106.22(10) ?
  Ba Al2 Pt2 12_555 . . 130.30(8) ?
  Ba Al2 Pt3 12_555 . . 73.52(6) ?
  Ba Al2 Al1 12_555 . . 126.18(12) ?
  Ba Al2 Al1 12_555 . 2_665 127.31(8) ?
  Ba Al2 Al2 12_555 . 22_555 67.18(9) ?
  Ba Al2 Al3 12_555 . 3_665 76.89(11) ?
  Ba Al2 Al4 12_555 . . 163.27(18) ?
  Ba Al2 Al4 12_555 . 7_555 108.36(12) ?
  Ba Al2 Al5 12_555 . 3_665 64.85(6) ?
  Ba Al2 Al5 12_555 . 15_555 77.59(6) ?
  Ba Al2 Al6 12_555 . . 115.66(9) ?
  Pt1 Al2 Pt2 3_665 . . 112.57(9) ?
  Pt1 Al2 Pt3 3_665 . . 109.91(9) ?
  Pt1 Al2 Al1 3_665 . . 116.84(11) ?
  Pt1 Al2 Al1 3_665 . 2_665 42.69(8) ?
  Pt1 Al2 Al2 3_665 . 22_555 60.34(9) ?
  Pt1 Al2 Al3 3_665 . 3_665 113.02(16) ?
  Pt1 Al2 Al4 3_665 . . 58.33(11) ?
  Pt1 Al2 Al4 3_665 . 7_555 40.07(7) ?
  Pt1 Al2 Al5 3_665 . 3_665 41.67(5) ?
  Pt1 Al2 Al5 3_665 . 15_555 56.46(8) ?
  Pt1 Al2 Al6 3_665 . . 82.43(7) ?
  Pt2 Al2 Pt3 . . . 118.04(14) ?
  Pt2 Al2 Al1 . . . 58.56(9) ?
  Pt2 Al2 Al1 . . 2_665 102.35(9) ?
  Pt2 Al2 Al2 . . 22_555 107.00(12) ?
  Pt2 Al2 Al3 . . 3_665 60.19(10) ?
  Pt2 Al2 Al4 . . . 59.16(9) ?
  Pt2 Al2 Al4 . . 7_555 84.41(8) ?
  Pt2 Al2 Al5 . . 3_665 147.55(12) ?
  Pt2 Al2 Al5 . . 15_555 150.85(13) ?
  Pt2 Al2 Al6 . . . 99.46(11) ?
  Pt3 Al2 Al1 . . . 62.80(11) ?
  Pt3 Al2 Al1 . . 2_665 80.85(9) ?
  Pt3 Al2 Al2 . . 22_555 132.94(12) ?
  Pt3 Al2 Al3 . . 3_665 132.97(13) ?
  Pt3 Al2 Al4 . . . 116.17(17) ?
  Pt3 Al2 Al4 . . 7_555 149.91(10) ?
  Pt3 Al2 Al5 . . 3_665 92.93(8) ?
  Pt3 Al2 Al5 . . 15_555 55.45(9) ?
  Pt3 Al2 Al6 . . . 45.34(8) ?
  Al1 Al2 Al1 . . 2_665 76.05(11) ?
  Al1 Al2 Al2 . . 22_555 164.20(13) ?
  Al1 Al2 Al3 . . 3_665 111.16(14) ?
  Al1 Al2 Al4 . . . 70.01(16) ?
  Al1 Al2 Al4 . . 7_555 125.28(11) ?
  Al1 Al2 Al5 . . 3_665 142.24(11) ?
  Al1 Al2 Al5 . . 15_555 100.07(14) ?
  Al1 Al2 Al6 . . . 46.41(8) ?
  Al1 Al2 Al2 2_665 . 22_555 103.03(12) ?
  Al1 Al2 Al3 2_665 . 3_665 145.68(13) ?
  Al1 Al2 Al4 2_665 . . 46.96(8) ?
  Al1 Al2 Al4 2_665 . 7_555 74.51(10) ?
  Al1 Al2 Al5 2_665 . 3_665 71.55(7) ?
  Al1 Al2 Al5 2_665 . 15_555 50.16(6) ?
  Al1 Al2 Al6 2_665 . . 41.35(8) ?
  Al2 Al2 Al3 22_555 . 3_665 60.73(13) ?
  Al2 Al2 Al4 22_555 . . 97.60(17) ?
  Al2 Al2 Al4 22_555 . 7_555 41.47(9) ?
  Al2 Al2 Al5 22_555 . 3_665 47.38(8) ?
  Al2 Al2 Al5 22_555 . 15_555 90.83(13) ?
  Al2 Al2 Al6 22_555 . . 140.25(10) ?
  Al3 Al2 Al4 3_665 . . 102.30(14) ?
  Al3 Al2 Al4 3_665 . 7_555 74.51(13) ?
  Al3 Al2 Al5 3_665 . 3_665 106.52(15) ?
  Al3 Al2 Al5 3_665 . 15_555 147.51(18) ?
  Al3 Al2 Al6 3_665 . . 157.54(16) ?
  Al4 Al2 Al4 . . 7_555 56.13(15) ?
  Al4 Al2 Al5 . . 3_665 100.00(13) ?
  Al4 Al2 Al5 . . 15_555 96.44(10) ?
  Al4 Al2 Al6 . . . 71.14(13) ?
  Al4 Al2 Al5 7_555 . 3_665 63.17(7) ?
  Al4 Al2 Al5 7_555 . 15_555 95.00(11) ?
  Al4 Al2 Al6 7_555 . . 115.35(9) ?
  Al5 Al2 Al5 3_665 . 15_555 43.46(10) ?
  Al5 Al2 Al6 3_665 . . 95.84(7) ?
  Al5 Al2 Al6 15_555 . . 54.52(9) ?
  Ba Al3 Ba 2_655 . 3_655 119.66(11) ?
  Ba Al3 Ba 2_655 . 11_655 68.40(6) ?
  Ba Al3 Pt2 2_655 . 2_655 170.89(12) ?
  Ba Al3 Pt2 2_655 . 9_655 68.896(18) ?
  Ba Al3 Pt4 2_655 . 1_655 73.48(7) ?
  Ba Al3 Al2 2_655 . 2_655 118.78(14) ?
  Ba Al3 Al2 2_655 . 24_655 68.67(7) ?
  Ba Al3 Al3 2_655 . 8_555 116.04(7) ?
  Ba Al3 Al7 2_655 . 2_655 61.56(7) ?
  Ba Al3 Al7 2_655 . 3_655 129.00(15) ?
  Ba Al3 Al9 2_655 . 1_655 61.12(6) ?
  Ba Al3 Ba 3_655 . 11_655 68.40(6) ?
  Ba Al3 Pt2 3_655 . 2_655 68.90(2) ?
  Ba Al3 Pt2 3_655 . 9_655 170.89(12) ?
  Ba Al3 Pt4 3_655 . 1_655 73.48(7) ?
  Ba Al3 Al2 3_655 . 2_655 68.67(11) ?
  Ba Al3 Al2 3_655 . 24_655 118.78(13) ?
  Ba Al3 Al3 3_655 . 8_555 116.04(7) ?
  Ba Al3 Al7 3_655 . 2_655 129.00(16) ?
  Ba Al3 Al7 3_655 . 3_655 61.56(7) ?
  Ba Al3 Al9 3_655 . 1_655 61.12(6) ?
  Ba Al3 Pt2 11_655 . 2_655 114.75(9) ?
  Ba Al3 Pt2 11_655 . 9_655 114.75(9) ?
  Ba Al3 Pt4 11_655 . 1_655 98.45(11) ?
  Ba Al3 Al2 11_655 . 2_655 59.82(9) ?
  Ba Al3 Al2 11_655 . 24_655 59.82(9) ?
  Ba Al3 Al3 11_655 . 8_555 166.22(16) ?
  Ba Al3 Al7 11_655 . 2_655 128.66(10) ?
  Ba Al3 Al7 11_655 . 3_655 128.66(11) ?
  Ba Al3 Al9 11_655 . 1_655 59.00(6) ?
  Pt2 Al3 Pt2 2_655 . 9_655 102.39(13) ?
  Pt2 Al3 Pt4 2_655 . 1_655 113.56(10) ?
  Pt2 Al3 Al2 2_655 . 2_655 59.81(9) ?
  Pt2 Al3 Al2 2_655 . 24_655 105.01(14) ?
  Pt2 Al3 Al3 2_655 . 8_555 58.82(8) ?
  Pt2 Al3 Al7 2_655 . 2_655 116.47(14) ?
  Pt2 Al3 Al7 2_655 . 3_655 56.58(10) ?
  Pt2 Al3 Al9 2_655 . 1_655 127.98(7) ?
  Pt2 Al3 Pt4 9_655 . 1_655 113.56(10) ?
  Pt2 Al3 Al2 9_655 . 2_655 105.01(16) ?
  Pt2 Al3 Al2 9_655 . 24_655 59.81(9) ?
  Pt2 Al3 Al3 9_655 . 8_555 58.82(8) ?
  Pt2 Al3 Al7 9_655 . 2_655 56.58(11) ?
  Pt2 Al3 Al7 9_655 . 3_655 116.47(15) ?
  Pt2 Al3 Al9 9_655 . 1_655 127.98(7) ?
  Pt4 Al3 Al2 1_655 . 2_655 141.17(14) ?
  Pt4 Al3 Al2 1_655 . 24_655 141.17(12) ?
  Pt4 Al3 Al3 1_655 . 8_555 95.34(15) ?
  Pt4 Al3 Al7 1_655 . 2_655 57.65(11) ?
  Pt4 Al3 Al7 1_655 . 3_655 57.65(12) ?
  Pt4 Al3 Al9 1_655 . 1_655 39.45(6) ?
  Al2 Al3 Al2 2_655 . 24_655 58.53(14) ?
  Al2 Al3 Al3 2_655 . 8_555 108.57(15) ?
  Al2 Al3 Al7 2_655 . 2_655 161.12(19) ?
  Al2 Al3 Al7 2_655 . 3_655 108.73(13) ?
  Al2 Al3 Al9 2_655 . 1_655 110.61(12) ?
  Al2 Al3 Al3 24_655 . 8_555 108.57(15) ?
  Al2 Al3 Al7 24_655 . 2_655 108.73(13) ?
  Al2 Al3 Al7 24_655 . 3_655 161.12(18) ?
  Al2 Al3 Al9 24_655 . 1_655 110.61(12) ?
  Al3 Al3 Al7 8_555 . 2_655 60.01(9) ?
  Al3 Al3 Al7 8_555 . 3_655 60.01(11) ?
  Al3 Al3 Al9 8_555 . 1_655 134.79(15) ?
  Al7 Al3 Al7 2_655 . 3_655 79.49(16) ?
  Al7 Al3 Al9 2_655 . 1_655 86.42(10) ?
  Al7 Al3 Al9 3_655 . 1_655 86.42(12) ?
  Pt1 Al4 Pt1 3_665 . 9_665 86.33(16) ?
  Pt1 Al4 Pt2 3_665 . . 116.41(12) ?
  Pt1 Al4 Pt5 3_665 . . 118.77(10) ?
  Pt1 Al4 Al1 3_665 . . 106.89(6) ?
  Pt1 Al4 Al1 3_665 . 2_665 57.61(11) ?
  Pt1 Al4 Al1 3_665 . 16_555 166.11(12) ?
  Pt1 Al4 Al1 3_665 . 17_665 102.01(14) ?
  Pt1 Al4 Al2 3_665 . . 60.82(9) ?
  Pt1 Al4 Al2 3_665 . 7_555 91.33(16) ?
  Pt1 Al4 Al2 3_665 . 16_555 132.2(2) ?
  Pt1 Al4 Al2 3_665 . 22_555 41.33(7) ?
  Pt1 Al4 Al4 3_665 . 7_555 49.96(10) ?
  Pt1 Al4 Al6 3_665 . . 81.14(5) ?
  Pt1 Al4 Al6 3_665 . 16_555 145.67(12) ?
  Pt1 Al4 Al8 3_665 . 3_665 51.74(9) ?
  Pt1 Al4 Pt2 9_665 . . 116.41(12) ?
  Pt1 Al4 Pt5 9_665 . . 118.77(10) ?
  Pt1 Al4 Al1 9_665 . . 166.11(12) ?
  Pt1 Al4 Al1 9_665 . 2_665 102.01(14) ?
  Pt1 Al4 Al1 9_665 . 16_555 106.89(6) ?
  Pt1 Al4 Al1 9_665 . 17_665 57.61(11) ?
  Pt1 Al4 Al2 9_665 . . 132.2(2) ?
  Pt1 Al4 Al2 9_665 . 7_555 41.33(7) ?
  Pt1 Al4 Al2 9_665 . 16_555 60.82(9) ?
  Pt1 Al4 Al2 9_665 . 22_555 91.33(16) ?
  Pt1 Al4 Al4 9_665 . 7_555 49.96(10) ?
  Pt1 Al4 Al6 9_665 . . 145.67(12) ?
  Pt1 Al4 Al6 9_665 . 16_555 81.14(5) ?
  Pt1 Al4 Al8 9_665 . 3_665 51.74(9) ?
  Pt2 Al4 Pt5 . . . 101.14(18) ?
  Pt2 Al4 Al1 . . . 54.22(9) ?
  Pt2 Al4 Al1 . . 2_665 141.07(14) ?
  Pt2 Al4 Al1 . . 16_555 54.22(9) ?
  Pt2 Al4 Al1 . . 17_665 141.07(14) ?
  Pt2 Al4 Al2 . . . 60.91(8) ?
  Pt2 Al4 Al2 . . 7_555 77.52(10) ?
  Pt2 Al4 Al2 . . 16_555 60.91(8) ?
  Pt2 Al4 Al2 . . 22_555 77.52(10) ?
  Pt2 Al4 Al4 . . 7_555 99.46(15) ?
  Pt2 Al4 Al6 . . . 97.75(12) ?
  Pt2 Al4 Al6 . . 16_555 97.75(12) ?
  Pt2 Al4 Al8 . . 3_665 159.5(2) ?
  Pt5 Al4 Al1 . . . 58.93(12) ?
  Pt5 Al4 Al1 . . 2_665 62.65(13) ?
  Pt5 Al4 Al1 . . 16_555 58.93(12) ?
  Pt5 Al4 Al1 . . 17_665 62.65(13) ?
  Pt5 Al4 Al2 . . . 107.76(16) ?
  Pt5 Al4 Al2 . . 7_555 145.33(7) ?
  Pt5 Al4 Al2 . . 16_555 107.76(16) ?
  Pt5 Al4 Al2 . . 22_555 145.33(7) ?
  Pt5 Al4 Al4 . . 7_555 159.40(14) ?
  Pt5 Al4 Al6 . . . 45.74(7) ?
  Pt5 Al4 Al6 . . 16_555 45.74(7) ?
  Pt5 Al4 Al8 . . 3_665 99.39(15) ?
  Al1 Al4 Al1 . . 2_665 89.00(13) ?
  Al1 Al4 Al1 . . 16_555 59.62(12) ?
  Al1 Al4 Al1 . . 17_665 121.5(2) ?
  Al1 Al4 Al2 . . . 55.43(12) ?
  Al1 Al4 Al2 . . 7_555 131.69(12) ?
  Al1 Al4 Al2 . . 16_555 105.94(16) ?
  Al1 Al4 Al2 . . 22_555 95.88(9) ?
  Al1 Al4 Al4 . . 7_555 136.76(12) ?
  Al1 Al4 Al6 . . . 44.26(7) ?
  Al1 Al4 Al6 . . 16_555 89.76(15) ?
  Al1 Al4 Al8 . . 3_665 140.57(12) ?
  Al1 Al4 Al1 2_665 . 16_555 121.5(2) ?
  Al1 Al4 Al1 2_665 . 17_665 65.87(11) ?
  Al1 Al4 Al2 2_665 . . 89.16(8) ?
  Al1 Al4 Al2 2_665 . 7_555 136.59(19) ?
  Al1 Al4 Al2 2_665 . 16_555 155.02(12) ?
  Al1 Al4 Al2 2_665 . 22_555 96.38(12) ?
  Al1 Al4 Al4 2_665 . 7_555 100.54(17) ?
  Al1 Al4 Al6 2_665 . . 44.76(9) ?
  Al1 Al4 Al6 2_665 . 16_555 93.94(14) ?
  Al1 Al4 Al8 2_665 . 3_665 51.83(13) ?
  Al1 Al4 Al1 16_555 . 17_665 89.00(13) ?
  Al1 Al4 Al2 16_555 . . 105.94(16) ?
  Al1 Al4 Al2 16_555 . 7_555 95.88(9) ?
  Al1 Al4 Al2 16_555 . 16_555 55.43(12) ?
  Al1 Al4 Al2 16_555 . 22_555 131.69(12) ?
  Al1 Al4 Al4 16_555 . 7_555 136.76(12) ?
  Al1 Al4 Al6 16_555 . . 89.76(15) ?
  Al1 Al4 Al6 16_555 . 16_555 44.26(7) ?
  Al1 Al4 Al8 16_555 . 3_665 140.57(12) ?
  Al1 Al4 Al2 17_665 . . 155.02(12) ?
  Al1 Al4 Al2 17_665 . 7_555 96.38(12) ?
  Al1 Al4 Al2 17_665 . 16_555 89.16(8) ?
  Al1 Al4 Al2 17_665 . 22_555 136.59(19) ?
  Al1 Al4 Al4 17_665 . 7_555 100.54(17) ?
  Al1 Al4 Al6 17_665 . . 93.94(14) ?
  Al1 Al4 Al6 17_665 . 16_555 44.76(9) ?
  Al1 Al4 Al8 17_665 . 3_665 51.83(13) ?
  Al2 Al4 Al2 . . 7_555 101.72(16) ?
  Al2 Al4 Al2 . . 16_555 115.78(15) ?
  Al2 Al4 Al2 . . 22_555 40.93(12) ?
  Al2 Al4 Al4 . . 7_555 82.40(15) ?
  Al2 Al4 Al6 . . . 66.81(10) ?
  Al2 Al4 Al6 . . 16_555 145.0(2) ?
  Al2 Al4 Al8 . . 3_665 112.32(14) ?
  Al2 Al4 Al2 7_555 . 16_555 40.93(12) ?
  Al2 Al4 Al2 7_555 . 22_555 68.93(10) ?
  Al2 Al4 Al4 7_555 . 7_555 41.47(8) ?
  Al2 Al4 Al6 7_555 . . 168.31(11) ?
  Al2 Al4 Al6 7_555 . 16_555 99.71(6) ?
  Al2 Al4 Al8 7_555 . 3_665 85.61(15) ?
  Al2 Al4 Al2 16_555 . 22_555 101.72(16) ?
  Al2 Al4 Al4 16_555 . 7_555 82.40(15) ?
  Al2 Al4 Al6 16_555 . . 145.0(2) ?
  Al2 Al4 Al6 16_555 . 16_555 66.81(10) ?
  Al2 Al4 Al8 16_555 . 3_665 112.32(14) ?
  Al2 Al4 Al4 22_555 . 7_555 41.47(8) ?
  Al2 Al4 Al6 22_555 . . 99.71(6) ?
  Al2 Al4 Al6 22_555 . 16_555 168.31(11) ?
  Al2 Al4 Al8 22_555 . 3_665 85.61(15) ?
  Al4 Al4 Al6 7_555 . . 130.79(8) ?
  Al4 Al4 Al6 7_555 . 16_555 130.79(8) ?
  Al4 Al4 Al8 7_555 . 3_665 60.01(16) ?
  Al6 Al4 Al6 . . 16_555 91.48(13) ?
  Al6 Al4 Al8 . . 3_665 96.54(10) ?
  Al6 Al4 Al8 16_555 . 3_665 96.54(10) ?
  Ba Al5 Ba . . 11_655 139.94(9) ?
  Ba Al5 Pt1 . . . 66.62(3) ?
  Ba Al5 Pt1 . . 11_655 92.56(4) ?
  Ba Al5 Pt3 . . 14_555 62.67(5) ?
  Ba Al5 Pt3 . . 15_655 154.91(11) ?
  Ba Al5 Al1 . . 15_655 137.51(9) ?
  Ba Al5 Al1 . . 22_555 56.75(6) ?
  Ba Al5 Al2 . . 2_655 99.69(6) ?
  Ba Al5 Al2 . . 12_555 50.78(5) ?
  Ba Al5 Al2 . . 14_555 56.71(6) ?
  Ba Al5 Al2 . . 24_655 122.61(6) ?
  Ba Al5 Al5 . . 13_655 69.97(6) ?
  Ba Al5 Al6 . . 13_665 115.23(10) ?
  Ba Al5 Al6 . . 22_555 100.93(8) ?
  Ba Al5 Pt1 11_655 . . 92.56(10) ?
  Ba Al5 Pt1 11_655 . 11_655 66.62(7) ?
  Ba Al5 Pt3 11_655 . 14_555 154.91(6) ?
  Ba Al5 Pt3 11_655 . 15_655 62.67(6) ?
  Ba Al5 Al1 11_655 . 15_655 56.75(10) ?
  Ba Al5 Al1 11_655 . 22_555 137.51(9) ?
  Ba Al5 Al2 11_655 . 2_655 50.78(6) ?
  Ba Al5 Al2 11_655 . 12_555 99.69(10) ?
  Ba Al5 Al2 11_655 . 14_555 122.61(9) ?
  Ba Al5 Al2 11_655 . 24_655 56.71(9) ?
  Ba Al5 Al5 11_655 . 13_655 69.97(10) ?
  Ba Al5 Al6 11_655 . 13_665 100.93(5) ?
  Ba Al5 Al6 11_655 . 22_555 115.23(5) ?
  Pt1 Al5 Pt1 . . 11_655 118.11(12) ?
  Pt1 Al5 Pt3 . . 14_555 110.15(7) ?
  Pt1 Al5 Pt3 . . 15_655 109.03(6) ?
  Pt1 Al5 Al1 . . 15_655 149.26(17) ?
  Pt1 Al5 Al1 . . 22_555 54.86(7) ?
  Pt1 Al5 Al2 . . 2_655 42.02(7) ?
  Pt1 Al5 Al2 . . 12_555 92.67(7) ?
  Pt1 Al5 Al2 . . 14_555 121.93(8) ?
  Pt1 Al5 Al2 . . 24_655 57.05(7) ?
  Pt1 Al5 Al5 . . 13_655 59.06(6) ?
  Pt1 Al5 Al6 . . 13_665 146.91(11) ?
  Pt1 Al5 Al6 . . 22_555 94.98(7) ?
  Pt1 Al5 Pt3 11_655 . 14_555 109.03(7) ?
  Pt1 Al5 Pt3 11_655 . 15_655 110.15(6) ?
  Pt1 Al5 Al1 11_655 . 15_655 54.86(5) ?
  Pt1 Al5 Al1 11_655 . 22_555 149.26(8) ?
  Pt1 Al5 Al2 11_655 . 2_655 92.67(11) ?
  Pt1 Al5 Al2 11_655 . 12_555 42.02(5) ?
  Pt1 Al5 Al2 11_655 . 14_555 57.05(9) ?
  Pt1 Al5 Al2 11_655 . 24_655 121.93(16) ?
  Pt1 Al5 Al5 11_655 . 13_655 59.06(6) ?
  Pt1 Al5 Al6 11_655 . 13_665 94.98(7) ?
  Pt1 Al5 Al6 11_655 . 22_555 146.91(11) ?
  Pt3 Al5 Pt3 14_555 . 15_655 98.63(11) ?
  Pt3 Al5 Al1 14_555 . 15_655 99.78(12) ?
  Pt3 Al5 Al1 14_555 . 22_555 58.01(9) ?
  Pt3 Al5 Al2 14_555 . 2_655 151.85(5) ?
  Pt3 Al5 Al2 14_555 . 12_555 90.07(9) ?
  Pt3 Al5 Al2 14_555 . 14_555 53.93(10) ?
  Pt3 Al5 Al2 14_555 . 24_655 127.42(12) ?
  Pt3 Al5 Al5 14_555 . 13_655 130.68(9) ?
  Pt3 Al5 Al6 14_555 . 13_665 54.12(7) ?
  Pt3 Al5 Al6 14_555 . 22_555 54.12(7) ?
  Pt3 Al5 Al1 15_655 . 15_655 58.01(7) ?
  Pt3 Al5 Al1 15_655 . 22_555 99.78(8) ?
  Pt3 Al5 Al2 15_655 . 2_655 90.07(9) ?
  Pt3 Al5 Al2 15_655 . 12_555 151.85(6) ?
  Pt3 Al5 Al2 15_655 . 14_555 127.42(11) ?
  Pt3 Al5 Al2 15_655 . 24_655 53.93(7) ?
  Pt3 Al5 Al5 15_655 . 13_655 130.68(15) ?
  Pt3 Al5 Al6 15_655 . 13_665 54.12(5) ?
  Pt3 Al5 Al6 15_655 . 22_555 54.12(5) ?
  Al1 Al5 Al1 15_655 . 22_555 147.95(14) ?
  Al1 Al5 Al2 15_655 . 2_655 107.48(14) ?
  Al1 Al5 Al2 15_655 . 12_555 94.22(7) ?
  Al1 Al5 Al2 15_655 . 14_555 81.37(10) ?
  Al1 Al5 Al2 15_655 . 24_655 99.10(12) ?
  Al1 Al5 Al5 15_655 . 13_655 106.03(11) ?
  Al1 Al5 Al6 15_655 . 13_665 51.87(9) ?
  Al1 Al5 Al6 15_655 . 22_555 96.95(10) ?
  Al1 Al5 Al2 22_555 . 2_655 94.22(9) ?
  Al1 Al5 Al2 22_555 . 12_555 107.48(8) ?
  Al1 Al5 Al2 22_555 . 14_555 99.10(13) ?
  Al1 Al5 Al2 22_555 . 24_655 81.37(10) ?
  Al1 Al5 Al5 22_555 . 13_655 106.03(7) ?
  Al1 Al5 Al6 22_555 . 13_665 96.95(13) ?
  Al1 Al5 Al6 22_555 . 22_555 51.87(8) ?
  Al2 Al5 Al2 2_655 . 12_555 94.75(10) ?
  Al2 Al5 Al2 2_655 . 14_555 136.54(12) ?
  Al2 Al5 Al2 2_655 . 24_655 41.79(10) ?
  Al2 Al5 Al5 2_655 . 13_655 47.38(8) ?
  Al2 Al5 Al6 2_655 . 13_665 143.78(7) ?
  Al2 Al5 Al6 2_655 . 22_555 114.26(7) ?
  Al2 Al5 Al2 12_555 . 14_555 41.79(11) ?
  Al2 Al5 Al2 12_555 . 24_655 136.54(15) ?
  Al2 Al5 Al5 12_555 . 13_655 47.38(8) ?
  Al2 Al5 Al6 12_555 . 13_665 114.26(9) ?
  Al2 Al5 Al6 12_555 . 22_555 143.78(13) ?
  Al2 Al5 Al2 14_555 . 24_655 178.33(17) ?
  Al2 Al5 Al5 14_555 . 13_655 89.17(10) ?
  Al2 Al5 Al6 14_555 . 13_665 75.17(10) ?
  Al2 Al5 Al6 14_555 . 22_555 106.39(15) ?
  Al2 Al5 Al5 24_655 . 13_655 89.17(14) ?
  Al2 Al5 Al6 24_655 . 13_665 106.39(9) ?
  Al2 Al5 Al6 24_655 . 22_555 75.17(10) ?
  Al5 Al5 Al6 13_655 . 13_665 154.03(7) ?
  Al5 Al5 Al6 13_655 . 22_555 154.03(7) ?
  Al6 Al5 Al6 13_665 . 22_555 51.94(10) ?
  Pt3 Al6 Pt3 . . 2_665 95.56(9) ?
  Pt3 Al6 Pt3 . . 3_565 95.56(9) ?
  Pt3 Al6 Pt5 . . . 121.22(7) ?
  Pt3 Al6 Al1 . . . 62.01(6) ?
  Pt3 Al6 Al1 . . 2_665 107.41(9) ?
  Pt3 Al6 Al1 . . 3_565 148.74(9) ?
  Pt3 Al6 Al2 . . . 42.98(4) ?
  Pt3 Al6 Al2 . . 2_665 136.04(9) ?
  Pt3 Al6 Al2 . . 3_565 101.46(5) ?
  Pt3 Al6 Al4 . . . 84.84(6) ?
  Pt3 Al6 Al4 . . 2_665 158.42(12) ?
  Pt3 Al6 Al4 . . 3_565 105.89(6) ?
  Pt3 Al6 Al5 . . 13_665 122.80(13) ?
  Pt3 Al6 Al5 . . 14_565 52.31(9) ?
  Pt3 Al6 Al5 . . 15_555 52.31(6) ?
  Pt3 Al6 Al6 . . 10_665 58.78(7) ?
  Pt3 Al6 Pt3 2_665 . 3_565 95.56(9) ?
  Pt3 Al6 Pt5 2_665 . . 121.22(7) ?
  Pt3 Al6 Al1 2_665 . . 148.74(9) ?
  Pt3 Al6 Al1 2_665 . 2_665 62.01(6) ?
  Pt3 Al6 Al1 2_665 . 3_565 107.41(7) ?
  Pt3 Al6 Al2 2_665 . . 101.46(6) ?
  Pt3 Al6 Al2 2_665 . 2_665 42.98(5) ?
  Pt3 Al6 Al2 2_665 . 3_565 136.04(8) ?
  Pt3 Al6 Al4 2_665 . . 105.89(7) ?
  Pt3 Al6 Al4 2_665 . 2_665 84.84(6) ?
  Pt3 Al6 Al4 2_665 . 3_565 158.42(9) ?
  Pt3 Al6 Al5 2_665 . 13_665 52.31(7) ?
  Pt3 Al6 Al5 2_665 . 14_565 122.80(13) ?
  Pt3 Al6 Al5 2_665 . 15_555 52.31(5) ?
  Pt3 Al6 Al6 2_665 . 10_665 58.78(7) ?
  Pt3 Al6 Pt5 3_565 . . 121.22(7) ?
  Pt3 Al6 Al1 3_565 . . 107.41(8) ?
  Pt3 Al6 Al1 3_565 . 2_665 148.74(8) ?
  Pt3 Al6 Al1 3_565 . 3_565 62.01(8) ?
  Pt3 Al6 Al2 3_565 . . 136.04(8) ?
  Pt3 Al6 Al2 3_565 . 2_665 101.46(8) ?
  Pt3 Al6 Al2 3_565 . 3_565 42.98(4) ?
  Pt3 Al6 Al4 3_565 . . 158.42(10) ?
  Pt3 Al6 Al4 3_565 . 2_665 105.89(11) ?
  Pt3 Al6 Al4 3_565 . 3_565 84.84(9) ?
  Pt3 Al6 Al5 3_565 . 13_665 52.31(5) ?
  Pt3 Al6 Al5 3_565 . 14_565 52.31(9) ?
  Pt3 Al6 Al5 3_565 . 15_555 122.80(13) ?
  Pt3 Al6 Al6 3_565 . 10_665 58.78(7) ?
  Pt5 Al6 Al1 . . . 63.88(9) ?
  Pt5 Al6 Al1 . . 2_665 63.88(9) ?
  Pt5 Al6 Al1 . . 3_565 63.88(10) ?
  Pt5 Al6 Al2 . . . 83.10(7) ?
  Pt5 Al6 Al2 . . 2_665 83.10(7) ?
  Pt5 Al6 Al2 . . 3_565 83.10(7) ?
  Pt5 Al6 Al4 . . . 44.26(7) ?
  Pt5 Al6 Al4 . . 2_665 44.26(6) ?
  Pt5 Al6 Al4 . . 3_565 44.26(8) ?
  Pt5 Al6 Al5 . . 13_665 115.97(7) ?
  Pt5 Al6 Al5 . . 14_565 115.97(7) ?
  Pt5 Al6 Al5 . . 15_555 115.97(7) ?
  Pt5 Al6 Al6 . . 10_665 180 ?
  Al1 Al6 Al1 . . 2_665 102.08(13) ?
  Al1 Al6 Al1 . . 3_565 102.08(13) ?
  Al1 Al6 Al2 . . . 47.30(10) ?
  Al1 Al6 Al2 . . 2_665 144.09(14) ?
  Al1 Al6 Al2 . . 3_565 73.11(10) ?
  Al1 Al6 Al4 . . . 53.91(10) ?
  Al1 Al6 Al4 . . 2_665 108.04(13) ?
  Al1 Al6 Al4 . . 3_565 48.20(11) ?
  Al1 Al6 Al5 . . 13_665 157.84(10) ?
  Al1 Al6 Al5 . . 14_565 62.22(8) ?
  Al1 Al6 Al5 . . 15_555 96.79(9) ?
  Al1 Al6 Al6 . . 10_665 116.12(9) ?
  Al1 Al6 Al1 2_665 . 3_565 102.08(15) ?
  Al1 Al6 Al2 2_665 . . 73.11(10) ?
  Al1 Al6 Al2 2_665 . 2_665 47.30(11) ?
  Al1 Al6 Al2 2_665 . 3_565 144.09(14) ?
  Al1 Al6 Al4 2_665 . . 48.20(10) ?
  Al1 Al6 Al4 2_665 . 2_665 53.91(14) ?
  Al1 Al6 Al4 2_665 . 3_565 108.04(15) ?
  Al1 Al6 Al5 2_665 . 13_665 96.79(8) ?
  Al1 Al6 Al5 2_665 . 14_565 157.84(12) ?
  Al1 Al6 Al5 2_665 . 15_555 62.22(10) ?
  Al1 Al6 Al6 2_665 . 10_665 116.12(9) ?
  Al1 Al6 Al2 3_565 . . 144.09(14) ?
  Al1 Al6 Al2 3_565 . 2_665 73.11(11) ?
  Al1 Al6 Al2 3_565 . 3_565 47.30(9) ?
  Al1 Al6 Al4 3_565 . . 108.04(14) ?
  Al1 Al6 Al4 3_565 . 2_665 48.20(14) ?
  Al1 Al6 Al4 3_565 . 3_565 53.91(10) ?
  Al1 Al6 Al5 3_565 . 13_665 62.22(7) ?
  Al1 Al6 Al5 3_565 . 14_565 96.79(12) ?
  Al1 Al6 Al5 3_565 . 15_555 157.84(9) ?
  Al1 Al6 Al6 3_565 . 10_665 116.12(10) ?
  Al2 Al6 Al2 . . 2_665 118.58(9) ?
  Al2 Al6 Al2 . . 3_565 118.58(7) ?
  Al2 Al6 Al4 . . . 42.05(6) ?
  Al2 Al6 Al4 . . 2_665 115.72(13) ?
  Al2 Al6 Al4 . . 3_565 92.89(10) ?
  Al2 Al6 Al5 . . 13_665 152.52(11) ?
  Al2 Al6 Al5 . . 14_565 84.80(10) ?
  Al2 Al6 Al5 . . 15_555 50.31(5) ?
  Al2 Al6 Al6 . . 10_665 96.90(7) ?
  Al2 Al6 Al2 2_665 . 3_565 118.58(9) ?
  Al2 Al6 Al4 2_665 . . 92.89(9) ?
  Al2 Al6 Al4 2_665 . 2_665 42.05(7) ?
  Al2 Al6 Al4 2_665 . 3_565 115.72(10) ?
  Al2 Al6 Al5 2_665 . 13_665 50.31(7) ?
  Al2 Al6 Al5 2_665 . 14_565 152.52(12) ?
  Al2 Al6 Al5 2_665 . 15_555 84.80(9) ?
  Al2 Al6 Al6 2_665 . 10_665 96.90(7) ?
  Al2 Al6 Al4 3_565 . . 115.72(11) ?
  Al2 Al6 Al4 3_565 . 2_665 92.89(11) ?
  Al2 Al6 Al4 3_565 . 3_565 42.05(10) ?
  Al2 Al6 Al5 3_565 . 13_665 84.80(7) ?
  Al2 Al6 Al5 3_565 . 14_565 50.31(9) ?
  Al2 Al6 Al5 3_565 . 15_555 152.52(10) ?
  Al2 Al6 Al6 3_565 . 10_665 96.90(7) ?
  Al4 Al6 Al4 . . 2_665 74.37(12) ?
  Al4 Al6 Al4 . . 3_565 74.37(13) ?
  Al4 Al6 Al5 . . 13_665 142.99(8) ?
  Al4 Al6 Al5 . . 14_565 114.59(9) ?
  Al4 Al6 Al5 . . 15_555 74.12(7) ?
  Al4 Al6 Al6 . . 10_665 135.74(7) ?
  Al4 Al6 Al4 2_665 . 3_565 74.37(10) ?
  Al4 Al6 Al5 2_665 . 13_665 74.12(8) ?
  Al4 Al6 Al5 2_665 . 14_565 142.99(13) ?
  Al4 Al6 Al5 2_665 . 15_555 114.59(11) ?
  Al4 Al6 Al6 2_665 . 10_665 135.74(6) ?
  Al4 Al6 Al5 3_565 . 13_665 114.59(10) ?
  Al4 Al6 Al5 3_565 . 14_565 74.12(8) ?
  Al4 Al6 Al5 3_565 . 15_555 142.99(10) ?
  Al4 Al6 Al6 3_565 . 10_665 135.74(8) ?
  Al5 Al6 Al5 13_665 . 14_565 102.26(10) ?
  Al5 Al6 Al5 13_665 . 15_555 102.26(9) ?
  Al5 Al6 Al6 13_665 . 10_665 64.03(7) ?
  Al5 Al6 Al5 14_565 . 15_555 102.26(12) ?
  Al5 Al6 Al6 14_565 . 10_665 64.03(7) ?
  Al5 Al6 Al6 15_555 . 10_665 64.03(7) ?
  Ba Al7 Ba . . 8_555 126.02(17) ?
  Ba Al7 Pt2 . . 3_555 74.16(8) ?
  Ba Al7 Pt2 . . 7_555 74.16(8) ?
  Ba Al7 Pt4 . . . 78.41(2) ?
  Ba Al7 Pt4 . . 7_555 155.57(16) ?
  Ba Al7 Al3 . . 2_545 70.93(6) ?
  Ba Al7 Al3 . . 3_665 70.93(9) ?
  Ba Al7 Al3 . . 7_545 124.35(9) ?
  Ba Al7 Al3 . . 9_665 124.35(8) ?
  Ba Al7 Al7 . . 2_555 113.15(6) ?
  Ba Al7 Al7 . . 3_555 113.15(7) ?
  Ba Al7 Al8 . . . 63.01(8) ?
  Ba Al7 Pt2 8_555 . 3_555 74.16(8) ?
  Ba Al7 Pt2 8_555 . 7_555 74.16(8) ?
  Ba Al7 Pt4 8_555 . . 155.57(16) ?
  Ba Al7 Pt4 8_555 . 7_555 78.41(2) ?
  Ba Al7 Al3 8_555 . 2_545 124.35(9) ?
  Ba Al7 Al3 8_555 . 3_665 124.35(8) ?
  Ba Al7 Al3 8_555 . 7_545 70.93(6) ?
  Ba Al7 Al3 8_555 . 9_665 70.93(9) ?
  Ba Al7 Al7 8_555 . 2_555 113.15(6) ?
  Ba Al7 Al7 8_555 . 3_555 113.15(7) ?
  Ba Al7 Al8 8_555 . . 63.01(8) ?
  Pt2 Al7 Pt2 3_555 . 7_555 106.05(19) ?
  Pt2 Al7 Pt4 3_555 . . 118.05(4) ?
  Pt2 Al7 Pt4 3_555 . 7_555 118.05(4) ?
  Pt2 Al7 Al3 3_555 . 2_545 59.85(7) ?
  Pt2 Al7 Al3 3_555 . 3_665 144.78(15) ?
  Pt2 Al7 Al3 3_555 . 7_545 59.85(7) ?
  Pt2 Al7 Al3 3_555 . 9_665 144.78(15) ?
  Pt2 Al7 Al7 3_555 . 2_555 156.98(15) ?
  Pt2 Al7 Al7 3_555 . 3_555 96.98(11) ?
  Pt2 Al7 Al8 3_555 . . 53.02(10) ?
  Pt2 Al7 Pt4 7_555 . . 118.05(4) ?
  Pt2 Al7 Pt4 7_555 . 7_555 118.05(4) ?
  Pt2 Al7 Al3 7_555 . 2_545 144.78(14) ?
  Pt2 Al7 Al3 7_555 . 3_665 59.85(8) ?
  Pt2 Al7 Al3 7_555 . 7_545 144.78(14) ?
  Pt2 Al7 Al3 7_555 . 9_665 59.85(8) ?
  Pt2 Al7 Al7 7_555 . 2_555 96.98(7) ?
  Pt2 Al7 Al7 7_555 . 3_555 156.98(17) ?
  Pt2 Al7 Al8 7_555 . . 53.02(10) ?
  Pt4 Al7 Pt4 . . 7_555 77.16(15) ?
  Pt4 Al7 Al3 . . 2_545 58.92(10) ?
  Pt4 Al7 Al3 . . 3_665 58.92(10) ?
  Pt4 Al7 Al3 . . 7_545 96.16(14) ?
  Pt4 Al7 Al3 . . 9_665 96.16(16) ?
  Pt4 Al7 Al7 . . 2_555 47.39(8) ?
  Pt4 Al7 Al7 . . 3_555 47.39(9) ?
  Pt4 Al7 Al8 . . . 141.42(7) ?
  Pt4 Al7 Al3 7_555 . 2_545 96.16(14) ?
  Pt4 Al7 Al3 7_555 . 3_665 96.16(16) ?
  Pt4 Al7 Al3 7_555 . 7_545 58.92(10) ?
  Pt4 Al7 Al3 7_555 . 9_665 58.92(10) ?
  Pt4 Al7 Al7 7_555 . 2_555 47.39(8) ?
  Pt4 Al7 Al7 7_555 . 3_555 47.39(9) ?
  Pt4 Al7 Al8 7_555 . . 141.42(7) ?
  Al3 Al7 Al3 2_545 . 3_665 111.30(14) ?
  Al3 Al7 Al3 2_545 . 7_545 59.99(11) ?
  Al3 Al7 Al3 2_545 . 9_665 149.7(2) ?
  Al3 Al7 Al7 2_545 . 2_555 100.73(16) ?
  Al3 Al7 Al7 2_545 . 3_555 50.25(11) ?
  Al3 Al7 Al8 2_545 . . 105.17(12) ?
  Al3 Al7 Al3 3_665 . 7_545 149.7(2) ?
  Al3 Al7 Al3 3_665 . 9_665 59.99(12) ?
  Al3 Al7 Al7 3_665 . 2_555 50.25(12) ?
  Al3 Al7 Al7 3_665 . 3_555 100.73(18) ?
  Al3 Al7 Al8 3_665 . . 105.17(14) ?
  Al3 Al7 Al3 7_545 . 9_665 111.30(14) ?
  Al3 Al7 Al7 7_545 . 2_555 100.73(16) ?
  Al3 Al7 Al7 7_545 . 3_555 50.25(11) ?
  Al3 Al7 Al8 7_545 . . 105.17(12) ?
  Al3 Al7 Al7 9_665 . 2_555 50.25(12) ?
  Al3 Al7 Al7 9_665 . 3_555 100.73(18) ?
  Al3 Al7 Al8 9_665 . . 105.17(14) ?
  Al7 Al7 Al7 2_555 . 3_555 60.00(14) ?
  Al7 Al7 Al8 2_555 . . 150.00(6) ?
  Al7 Al7 Al8 3_555 . . 150.00(11) ?
  Ba Al8 Ba . . 8_555 123.31(18) ?
  Ba Al8 Pt1 . . . 76.767(17) ?
  Ba Al8 Pt1 . . 8_555 159.92(17) ?
  Ba Al8 Pt2 . . 3_555 73.54(9) ?
  Ba Al8 Pt2 . . 7_555 73.54(9) ?
  Ba Al8 Al1 . . 3_555 67.09(9) ?
  Ba Al8 Al1 . . 7_555 126.54(9) ?
  Ba Al8 Al1 . . 18_555 126.54(9) ?
  Ba Al8 Al1 . . 22_555 67.09(7) ?
  Ba Al8 Al4 . . 2_655 114.28(6) ?
  Ba Al8 Al4 . . 9_655 114.28(7) ?
  Ba Al8 Al7 . . . 61.65(9) ?
  Ba Al8 Pt1 8_555 . . 159.92(17) ?
  Ba Al8 Pt1 8_555 . 8_555 76.767(17) ?
  Ba Al8 Pt2 8_555 . 3_555 73.54(9) ?
  Ba Al8 Pt2 8_555 . 7_555 73.54(9) ?
  Ba Al8 Al1 8_555 . 3_555 126.54(9) ?
  Ba Al8 Al1 8_555 . 7_555 67.09(7) ?
  Ba Al8 Al1 8_555 . 18_555 67.09(9) ?
  Ba Al8 Al1 8_555 . 22_555 126.54(9) ?
  Ba Al8 Al4 8_555 . 2_655 114.28(6) ?
  Ba Al8 Al4 8_555 . 9_655 114.28(7) ?
  Ba Al8 Al7 8_555 . . 61.65(9) ?
  Pt1 Al8 Pt1 . . 8_555 83.16(17) ?
  Pt1 Al8 Pt2 . . 3_555 116.52(4) ?
  Pt1 Al8 Pt2 . . 7_555 116.52(3) ?
  Pt1 Al8 Al1 . . 3_555 57.75(10) ?
  Pt1 Al8 Al1 . . 7_555 102.05(16) ?
  Pt1 Al8 Al1 . . 18_555 102.05(17) ?
  Pt1 Al8 Al1 . . 22_555 57.75(10) ?
  Pt1 Al8 Al4 . . 2_655 49.62(9) ?
  Pt1 Al8 Al4 . . 9_655 49.62(11) ?
  Pt1 Al8 Al7 . . . 138.42(8) ?
  Pt1 Al8 Pt2 8_555 . 3_555 116.52(4) ?
  Pt1 Al8 Pt2 8_555 . 7_555 116.52(3) ?
  Pt1 Al8 Al1 8_555 . 3_555 102.05(17) ?
  Pt1 Al8 Al1 8_555 . 7_555 57.75(10) ?
  Pt1 Al8 Al1 8_555 . 18_555 57.75(10) ?
  Pt1 Al8 Al1 8_555 . 22_555 102.05(16) ?
  Pt1 Al8 Al4 8_555 . 2_655 49.62(9) ?
  Pt1 Al8 Al4 8_555 . 9_655 49.62(11) ?
  Pt1 Al8 Al7 8_555 . . 138.42(8) ?
  Pt2 Al8 Pt2 3_555 . 7_555 106.7(2) ?
  Pt2 Al8 Al1 3_555 . 3_555 59.19(8) ?
  Pt2 Al8 Al1 3_555 . 7_555 140.48(15) ?
  Pt2 Al8 Al1 3_555 . 18_555 59.19(8) ?
  Pt2 Al8 Al1 3_555 . 22_555 140.48(15) ?
  Pt2 Al8 Al4 3_555 . 2_655 96.65(9) ?
  Pt2 Al8 Al4 3_555 . 9_655 156.6(2) ?
  Pt2 Al8 Al7 3_555 . . 53.36(11) ?
  Pt2 Al8 Al1 7_555 . 3_555 140.48(16) ?
  Pt2 Al8 Al1 7_555 . 7_555 59.19(8) ?
  Pt2 Al8 Al1 7_555 . 18_555 140.48(16) ?
  Pt2 Al8 Al1 7_555 . 22_555 59.19(8) ?
  Pt2 Al8 Al4 7_555 . 2_655 156.63(17) ?
  Pt2 Al8 Al4 7_555 . 9_655 96.65(13) ?
  Pt2 Al8 Al7 7_555 . . 53.36(10) ?
  Al1 Al8 Al1 3_555 . 7_555 154.9(3) ?
  Al1 Al8 Al1 3_555 . 18_555 68.03(9) ?
  Al1 Al8 Al1 3_555 . 22_555 106.25(11) ?
  Al1 Al8 Al4 3_555 . 2_655 53.99(13) ?
  Al1 Al8 Al4 3_555 . 9_655 102.2(2) ?
  Al1 Al8 Al7 3_555 . . 102.54(15) ?
  Al1 Al8 Al1 7_555 . 18_555 106.25(11) ?
  Al1 Al8 Al1 7_555 . 22_555 68.03(9) ?
  Al1 Al8 Al4 7_555 . 2_655 102.23(18) ?
  Al1 Al8 Al4 7_555 . 9_655 53.99(14) ?
  Al1 Al8 Al7 7_555 . . 102.54(14) ?
  Al1 Al8 Al1 18_555 . 22_555 154.9(3) ?
  Al1 Al8 Al4 18_555 . 2_655 53.99(13) ?
  Al1 Al8 Al4 18_555 . 9_655 102.2(2) ?
  Al1 Al8 Al7 18_555 . . 102.54(15) ?
  Al1 Al8 Al4 22_555 . 2_655 102.23(18) ?
  Al1 Al8 Al4 22_555 . 9_655 53.99(14) ?
  Al1 Al8 Al7 22_555 . . 102.54(14) ?
  Al4 Al8 Al4 2_655 . 9_655 59.98(17) ?
  Al4 Al8 Al7 2_655 . . 150.01(9) ?
  Al4 Al8 Al7 9_655 . . 150.01(13) ?
  Ba Al9 Ba . . 2_555 112.108(8) ?
  Ba Al9 Ba . . 3_555 112.108(16) ?
  Ba Al9 Ba . . 10_555 67.892(8) ?
  Ba Al9 Ba . . 11_555 180 ?
  Ba Al9 Ba . . 12_555 67.892(16) ?
  Ba Al9 Pt4 . . . 73.315(10) ?
  Ba Al9 Pt4 . . 10_555 106.685(10) ?
  Ba Al9 Al3 . . 1_455 118.53(6) ?
  Ba Al9 Al3 . . 2_545 57.168(13) ?
  Ba Al9 Al3 . . 3_665 57.17(7) ?
  Ba Al9 Al3 . . 10_565 122.832(13) ?
  Ba Al9 Al3 . . 11_655 61.47(6) ?
  Ba Al9 Al3 . . 12_445 122.83(7) ?
  Ba Al9 Ba 2_555 . 3_555 112.108(16) ?
  Ba Al9 Ba 2_555 . 10_555 180 ?
  Ba Al9 Ba 2_555 . 11_555 67.892(8) ?
  Ba Al9 Ba 2_555 . 12_555 67.892(16) ?
  Ba Al9 Pt4 2_555 . . 73.315(10) ?
  Ba Al9 Pt4 2_555 . 10_555 106.685(10) ?
  Ba Al9 Al3 2_555 . 1_455 57.168(13) ?
  Ba Al9 Al3 2_555 . 2_545 118.53(6) ?
  Ba Al9 Al3 2_555 . 3_665 57.17(7) ?
  Ba Al9 Al3 2_555 . 10_565 61.47(6) ?
  Ba Al9 Al3 2_555 . 11_655 122.832(13) ?
  Ba Al9 Al3 2_555 . 12_445 122.83(7) ?
  Ba Al9 Ba 3_555 . 10_555 67.892(16) ?
  Ba Al9 Ba 3_555 . 11_555 67.892(16) ?
  Ba Al9 Ba 3_555 . 12_555 180 ?
  Ba Al9 Pt4 3_555 . . 73.315(10) ?
  Ba Al9 Pt4 3_555 . 10_555 106.685(10) ?
  Ba Al9 Al3 3_555 . 1_455 57.168(16) ?
  Ba Al9 Al3 3_555 . 2_545 57.168(16) ?
  Ba Al9 Al3 3_555 . 3_665 118.53(5) ?
  Ba Al9 Al3 3_555 . 10_565 122.832(16) ?
  Ba Al9 Al3 3_555 . 11_655 122.832(16) ?
  Ba Al9 Al3 3_555 . 12_445 61.47(5) ?
  Ba Al9 Ba 10_555 . 11_555 112.108(8) ?
  Ba Al9 Ba 10_555 . 12_555 112.108(16) ?
  Ba Al9 Pt4 10_555 . . 106.685(10) ?
  Ba Al9 Pt4 10_555 . 10_555 73.315(10) ?
  Ba Al9 Al3 10_555 . 1_455 122.832(13) ?
  Ba Al9 Al3 10_555 . 2_545 61.47(6) ?
  Ba Al9 Al3 10_555 . 3_665 122.83(7) ?
  Ba Al9 Al3 10_555 . 10_565 118.53(6) ?
  Ba Al9 Al3 10_555 . 11_655 57.168(13) ?
  Ba Al9 Al3 10_555 . 12_445 57.17(7) ?
  Ba Al9 Ba 11_555 . 12_555 112.108(16) ?
  Ba Al9 Pt4 11_555 . . 106.685(10) ?
  Ba Al9 Pt4 11_555 . 10_555 73.315(10) ?
  Ba Al9 Al3 11_555 . 1_455 61.47(6) ?
  Ba Al9 Al3 11_555 . 2_545 122.832(13) ?
  Ba Al9 Al3 11_555 . 3_665 122.83(7) ?
  Ba Al9 Al3 11_555 . 10_565 57.168(13) ?
  Ba Al9 Al3 11_555 . 11_655 118.53(6) ?
  Ba Al9 Al3 11_555 . 12_445 57.17(7) ?
  Ba Al9 Pt4 12_555 . . 106.685(10) ?
  Ba Al9 Pt4 12_555 . 10_555 73.315(10) ?
  Ba Al9 Al3 12_555 . 1_455 122.832(16) ?
  Ba Al9 Al3 12_555 . 2_545 122.832(16) ?
  Ba Al9 Al3 12_555 . 3_665 61.47(5) ?
  Ba Al9 Al3 12_555 . 10_565 57.168(16) ?
  Ba Al9 Al3 12_555 . 11_655 57.168(16) ?
  Ba Al9 Al3 12_555 . 12_445 118.53(5) ?
  Pt4 Al9 Pt4 . . 10_555 180 ?
  Pt4 Al9 Al3 . . 1_455 45.21(6) ?
  Pt4 Al9 Al3 . . 2_545 45.21(6) ?
  Pt4 Al9 Al3 . . 3_665 45.21(5) ?
  Pt4 Al9 Al3 . . 10_565 134.79(6) ?
  Pt4 Al9 Al3 . . 11_655 134.79(6) ?
  Pt4 Al9 Al3 . . 12_445 134.79(5) ?
  Pt4 Al9 Al3 10_555 . 1_455 134.79(6) ?
  Pt4 Al9 Al3 10_555 . 2_545 134.79(6) ?
  Pt4 Al9 Al3 10_555 . 3_665 134.79(5) ?
  Pt4 Al9 Al3 10_555 . 10_565 45.21(6) ?
  Pt4 Al9 Al3 10_555 . 11_655 45.21(6) ?
  Pt4 Al9 Al3 10_555 . 12_445 45.21(5) ?
  Al3 Al9 Al3 1_455 . 2_545 75.85(6) ?
  Al3 Al9 Al3 1_455 . 3_665 75.85(8) ?
  Al3 Al9 Al3 1_455 . 10_565 104.15(6) ?
  Al3 Al9 Al3 1_455 . 11_655 180 ?
  Al3 Al9 Al3 1_455 . 12_445 104.15(8) ?
  Al3 Al9 Al3 2_545 . 3_665 75.85(8) ?
  Al3 Al9 Al3 2_545 . 10_565 180 ?
  Al3 Al9 Al3 2_545 . 11_655 104.15(6) ?
  Al3 Al9 Al3 2_545 . 12_445 104.15(8) ?
  Al3 Al9 Al3 3_665 . 10_565 104.15(8) ?
  Al3 Al9 Al3 3_665 . 11_655 104.15(8) ?
  Al3 Al9 Al3 3_665 . 12_445 180 ?
  Al3 Al9 Al3 10_565 . 11_655 75.85(6) ?
  Al3 Al9 Al3 10_565 . 12_445 75.85(8) ?
  Al3 Al9 Al3 11_655 . 12_445 75.85(8) ?

loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion
 _geom_torsion_publ_flag
 ? ? ? ? ? ? ? ? ? ?

loop_
 _geom_hbond_atom_site_label_D
 _geom_hbond_atom_site_label_H
 _geom_hbond_atom_site_label_A
 _geom_hbond_site_symmetry_D
 _geom_hbond_site_symmetry_H
 _geom_hbond_site_symmetry_A
 _geom_hbond_distance_DH
 _geom_hbond_distance_HA
 _geom_hbond_distance_DA
 _geom_hbond_angle_DHA
 _geom_hbond_publ_flag
 ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST



